#------------------------------------------------------------------------------
#$Date: 2016-03-24 02:54:37 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179603 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/67/4506710.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4506710
loop_
_publ_author_name
'Cheng, Ping-Shing'
'Marivel, Samipillai'
'Zang, Shuang-Quan'
'Gao, Guang-Gang'
'Mak, Thomas C. W.'
_publ_section_title
;
 Argentophilic Infinite Chain, Column, and Layer Structures Assembled with
 the Multinuclear Silver(I)--Phenylethynide Supramolecular Synthon
;
_journal_issue                   9
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              4519
_journal_paper_doi               10.1021/cg300691n
_journal_volume                  12
_journal_year                    2012
_chemical_formula_moiety         'C36 H32 Ag5 F6 N0 O2 S2 Sb'
_chemical_formula_sum            'C36 H32 Ag5 F6 N0 O2 S2 Sb'
_chemical_formula_weight         1335.84
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                114.1130(10)
_cell_angle_beta                 99.0790(10)
_cell_angle_gamma                94.4240(10)
_cell_formula_units_Z            2
_cell_length_a                   8.4128(5)
_cell_length_b                   16.7218(11)
_cell_length_c                   16.7461(11)
_cell_measurement_temperature    293(2)
_cell_volume                     2096.9(2)
_computing_cell_refinement       SAINT(Bruker,2001)
_computing_data_collection       APEX2(Bruker,2003)
_computing_data_reduction        APEX2(Bruker,2003)
_computing_molecular_graphics    DIAMOND
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.976
_diffrn_measured_fraction_theta_max 0.976
_diffrn_measurement_device_type  'SMART CCD APEX II'
_diffrn_measurement_method       'ω and φ'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0333
_diffrn_reflns_av_sigmaI/netI    0.0264
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            43059
_diffrn_reflns_theta_full        26.00
_diffrn_reflns_theta_max         26.00
_diffrn_reflns_theta_min         1.36
_exptl_absorpt_coefficient_mu    3.080
_exptl_absorpt_correction_T_max  0.5779
_exptl_absorpt_correction_T_min  0.3722
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.116
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             1272
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.20
_refine_diff_density_max         1.304
_refine_diff_density_min         -0.971
_refine_diff_density_rms         0.142
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.092
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     502
_refine_ls_number_reflns         8059
_refine_ls_number_restraints     5
_refine_ls_restrained_S_all      1.092
_refine_ls_R_factor_all          0.0873
_refine_ls_R_factor_gt           0.0675
_refine_ls_shift/su_max          0.009
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0348P)²+27.8259P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1498
_refine_ls_wR_factor_ref         0.1614
_reflns_number_gt                6258
_reflns_number_total             8059
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg300691n_si_001.cif
_cod_data_source_block           3e
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4506710
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ag1 Ag 0.59512(9) 0.55094(5) -0.05698(5) 0.0507(2) Uani 1 1 d .
Ag2 Ag 0.85735(10) 0.42270(6) -0.08959(5) 0.0530(2) Uani 1 1 d .
Ag3 Ag 0.94916(11) 0.61764(6) -0.05060(6) 0.0609(2) Uani 1 1 d .
Ag4 Ag 0.50755(11) 0.64515(6) 0.11863(6) 0.0626(3) Uani 1 1 d .
Ag5 Ag 0.7976(13) 0.5278(8) 0.0975(6) 0.065(2) Uani 0.35(4) 1 d P
Ag5' Ag 0.8069(9) 0.5106(11) 0.1047(6) 0.0960(19) Uani 0.65(4) 1 d P
C1 C 0.5757(12) 0.5380(7) 0.1699(7) 0.050(2) Uani 1 1 d .
C2 C 0.6576(13) 0.5846(8) 0.2409(8) 0.061(3) Uani 1 1 d .
C3 C 0.7468(10) 0.6406(5) 0.3308(4) 0.059(3) Uani 1 1 d G
C4 C 0.6963(11) 0.6318(6) 0.4023(6) 0.094(5) Uani 1 1 d G
H4 H 0.6113 0.5874 0.3918 0.112 Uiso 1 1 calc R
C5 C 0.7728(14) 0.6893(8) 0.4895(5) 0.103(5) Uani 1 1 d G
H5 H 0.7390 0.6834 0.5373 0.124 Uiso 1 1 calc R
C6 C 0.8998(13) 0.7557(7) 0.5052(4) 0.100(5) Uani 1 1 d G
H6 H 0.9510 0.7941 0.5635 0.119 Uiso 1 1 calc R
C7 C 0.9504(12) 0.7645(6) 0.4336(6) 0.117(7) Uani 1 1 d G
H7 H 1.0354 0.8089 0.4441 0.141 Uiso 1 1 calc R
C8 C 0.8739(11) 0.7070(6) 0.3464(5) 0.090(4) Uani 1 1 d G
H8 H 0.9077 0.7129 0.2986 0.108 Uiso 1 1 calc R
C9 C 0.7605(12) 0.6504(7) 0.0487(7) 0.050(2) Uani 1 1 d .
C10 C 0.8380(13) 0.7254(8) 0.0914(7) 0.055(3) Uani 1 1 d .
C11 C 0.9219(9) 0.8137(4) 0.1494(5) 0.062(3) Uani 1 1 d G
C12 C 0.8723(10) 0.8642(6) 0.2278(6) 0.083(4) Uani 1 1 d G
H12 H 0.7878 0.8399 0.2448 0.099 Uiso 1 1 calc R
C13 C 0.9490(13) 0.9510(6) 0.2808(6) 0.106(6) Uani 1 1 d G
H13 H 0.9159 0.9847 0.3332 0.127 Uiso 1 1 calc R
C14 C 1.0754(13) 0.9872(4) 0.2554(7) 0.110(6) Uani 1 1 d G
H14 H 1.1267 1.0453 0.2909 0.131 Uiso 1 1 calc R
C15 C 1.1250(11) 0.9367(6) 0.1770(8) 0.108(6) Uani 1 1 d G
H15 H 1.2095 0.9610 0.1600 0.129 Uiso 1 1 calc R
C16 C 1.0482(11) 0.8500(5) 0.1240(6) 0.081(4) Uani 1 1 d G
H16 H 1.0814 0.8162 0.0715 0.097 Uiso 1 1 calc R
C17 C 0.7540(12) 0.3589(7) -0.0231(7) 0.051(2) Uani 1 1 d .
C18 C 0.6741(15) 0.3027(8) -0.0149(7) 0.063(3) Uani 1 1 d .
C19 C 0.5843(15) 0.2350(6) 0.0035(7) 0.083(4) Uani 1 1 d G
C20 C 0.4979(14) 0.1586(6) -0.0683(6) 0.080(4) Uani 1 1 d G
H20 H 0.4988 0.1506 -0.1266 0.096 Uiso 1 1 calc R
C21 C 0.4101(16) 0.0942(7) -0.0531(9) 0.118(6) Uani 1 1 d G
H21 H 0.3523 0.0431 -0.1011 0.141 Uiso 1 1 calc R
C22 C 0.409(3) 0.1062(11) 0.0339(11) 0.24(2) Uani 1 1 d G
H22 H 0.3499 0.0631 0.0441 0.284 Uiso 1 1 calc R
C23 C 0.495(3) 0.1826(13) 0.1057(8) 0.40(4) Uani 1 1 d G
H23 H 0.4941 0.1906 0.1640 0.485 Uiso 1 1 calc R
C24 C 0.583(3) 0.2470(10) 0.0905(6) 0.24(2) Uani 1 1 d G
H24 H 0.6407 0.2981 0.1386 0.285 Uiso 1 1 calc R
C25 C 0.9366(13) 0.4748(8) -0.1734(7) 0.058(3) Uani 1 1 d D
C26 C 0.958(3) 0.4869(15) -0.2370(15) 0.048(6) Uani 0.487(14) 1 d P
C27 C 0.960(2) 0.4933(11) -0.3177(10) 0.056(6) Uani 0.487(14) 1 d PG
C28 C 0.862(2) 0.4334(12) -0.3987(12) 0.089(10) Uani 0.487(14) 1 d PG
C29 C 0.866(3) 0.4453(17) -0.4759(10) 0.099(11) Uani 0.487(14) 1 d PG
C30 C 0.967(4) 0.5171(19) -0.4721(14) 0.123(15) Uani 0.487(14) 1 d PG
C31 C 1.065(3) 0.5770(15) -0.3911(18) 0.18(3) Uani 0.487(14) 1 d PG
H31 H 1.1323 0.6250 -0.3885 0.214 Uiso 0.487(14) 1 calc PR
C32 C 1.061(3) 0.5651(12) -0.3139(13) 0.115(14) Uani 0.487(14) 1 d PG
H32 H 1.1268 0.6052 -0.2597 0.138 Uiso 0.487(14) 1 calc PR
C26' C 0.860(3) 0.4883(14) -0.2332(12) 0.053(6) Uani 0.513(14) 1 d PD
C27' C 0.7488(17) 0.5037(12) -0.3053(10) 0.057(6) Uani 0.513(14) 1 d PG
C28' C 0.745(2) 0.4442(12) -0.3928(12) 0.095(11) Uani 0.513(14) 1 d PG
C29' C 0.650(3) 0.4532(16) -0.4635(9) 0.125(15) Uani 0.513(14) 1 d PG
C30' C 0.558(2) 0.5218(18) -0.4467(14) 0.091(10) Uani 0.513(14) 1 d PG
C31' C 0.562(2) 0.5814(13) -0.3591(17) 0.124(16) Uani 0.513(14) 1 d PG
H31' H 0.5005 0.6273 -0.3478 0.148 Uiso 0.513(14) 1 calc PR
C32' C 0.657(2) 0.5723(11) -0.2884(11) 0.097(11) Uani 0.513(14) 1 d PG
H32' H 0.6594 0.6122 -0.2298 0.116 Uiso 0.513(14) 1 calc PR
O1 O 0.5076(15) 0.7772(6) 0.2414(6) 0.096(3) Uani 1 1 d .
S1 S 0.4666(11) 0.7881(4) 0.3282(5) 0.087(3) Uani 0.67(2) 1 d PD
S1' S 0.385(3) 0.8079(18) 0.2942(13) 0.151(10) Uani 0.33(2) 1 d P
C33 C 0.575(6) 0.8917(18) 0.4057(16) 0.26(2) Uani 1 1 d .
C34 C 0.283(3) 0.828(3) 0.334(2) 0.27(2) Uani 1 1 d D
O2 O 0.9645(16) 0.7160(8) -0.1124(8) 0.110(4) Uani 1 1 d D
S2 S 1.046(3) 0.7559(9) -0.1613(8) 0.232(11) Uani 0.55 1 d PD
S2' S 0.823(2) 0.7525(9) -0.1419(10) 0.153(6) Uani 0.45 1 d P
C35 C 1.110(7) 0.8692(11) -0.111(3) 0.33(3) Uani 1 1 d D
C36 C 0.905(5) 0.797(5) -0.215(7) 0.60(8) Uani 1 1 d D
Sb1 Sb 0.57639(14) 0.14256(8) 0.35267(7) 0.0924(3) Uani 1 1 d .
F1 F 0.637(3) 0.2452(13) 0.4516(13) 0.287(12) Uani 1 1 d .
F2 F 0.7243(19) 0.1026(12) 0.4187(12) 0.203(7) Uani 1 1 d .
F3 F 0.417(2) 0.1081(15) 0.3994(11) 0.242(9) Uani 1 1 d .
F4 F 0.523(2) 0.0425(16) 0.2583(14) 0.354(19) Uani 1 1 d .
F5 F 0.416(3) 0.180(2) 0.304(2) 0.353(17) Uani 1 1 d .
F6 F 0.730(3) 0.176(2) 0.3121(14) 0.44(3) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
C9 Ag1 C1 173.0(4) . 2_665
C9 Ag1 Ag4 59.1(3) . .
C1 Ag1 Ag4 122.3(3) 2_665 .
C9 Ag1 Ag4 135.8(3) . 2_665
C1 Ag1 Ag4 51.1(3) 2_665 2_665
Ag4 Ag1 Ag4 108.05(3) . 2_665
C9 Ag1 Ag3 51.6(3) . .
C1 Ag1 Ag3 126.8(3) 2_665 .
Ag4 Ag1 Ag3 110.64(3) . .
Ag4 Ag1 Ag3 118.41(4) 2_665 .
C9 Ag1 Ag5 55.2(4) . .
C1 Ag1 Ag5 131.8(4) 2_665 .
Ag4 Ag1 Ag5 64.9(2) . .
Ag4 Ag1 Ag5 80.8(2) 2_665 .
Ag3 Ag1 Ag5 74.8(2) . .
C9 Ag1 Ag2 90.8(3) . .
C1 Ag1 Ag2 93.4(3) 2_665 .
Ag4 Ag1 Ag2 123.63(4) . .
Ag4 Ag1 Ag2 59.93(3) 2_665 .
Ag3 Ag1 Ag2 58.94(3) . .
Ag5 Ag1 Ag2 58.9(2) . .
C9 Ag1 Ag5 135.9(3) . 2_665
C1 Ag1 Ag5 45.1(3) 2_665 2_665
Ag4 Ag1 Ag5 77.27(18) . 2_665
Ag4 Ag1 Ag5 60.94(18) 2_665 2_665
Ag3 Ag1 Ag5 171.03(15) . 2_665
Ag5 Ag1 Ag5 113.2(2) . 2_665
Ag2 Ag1 Ag5 120.83(18) . 2_665
C9 Ag1 Ag5' 135.1(3) . 2_665
C1 Ag1 Ag5' 44.9(3) 2_665 2_665
Ag4 Ag1 Ag5' 77.68(11) . 2_665
Ag4 Ag1 Ag5' 66.3(3) 2_665 2_665
Ag3 Ag1 Ag5' 166.7(3) . 2_665
Ag5 Ag1 Ag5' 118.5(4) . 2_665
Ag2 Ag1 Ag5' 125.9(3) . 2_665
Ag5 Ag1 Ag5' 6.3(4) 2_665 2_665
C17 Ag2 C25 171.7(4) . .
C17 Ag2 Ag3 56.7(3) . 2_765
C25 Ag2 Ag3 129.7(3) . 2_765
C17 Ag2 Ag5 133.0(3) . 2_765
C25 Ag2 Ag5 52.9(3) . 2_765
Ag3 Ag2 Ag5 76.84(12) 2_765 2_765
C17 Ag2 Ag5 59.3(4) . .
C25 Ag2 Ag5 126.6(4) . .
Ag3 Ag2 Ag5 66.20(14) 2_765 .
Ag5 Ag2 Ag5 110.5(2) 2_765 .
C17 Ag2 Ag3 133.9(3) . .
C25 Ag2 Ag3 51.8(3) . .
Ag3 Ag2 Ag3 110.41(3) 2_765 .
Ag5 Ag2 Ag3 65.9(2) 2_765 .
Ag5 Ag2 Ag3 74.85(19) . .
C17 Ag2 Ag4 53.5(3) . 2_665
C25 Ag2 Ag4 119.7(3) . 2_665
Ag3 Ag2 Ag4 110.24(3) 2_765 2_665
Ag5 Ag2 Ag4 169.61(19) 2_765 2_665
Ag5 Ag2 Ag4 79.7(2) . 2_665
Ag3 Ag2 Ag4 116.61(4) . 2_665
C17 Ag2 Ag5' 139.3(5) . 2_765
C25 Ag2 Ag5' 47.0(5) . 2_765
Ag3 Ag2 Ag5' 82.8(4) 2_765 2_765
Ag5 Ag2 Ag5' 6.8(4) 2_765 2_765
Ag5 Ag2 Ag5' 110.5(3) . 2_765
Ag3 Ag2 Ag5' 60.0(4) . 2_765
Ag4 Ag2 Ag5' 166.3(3) 2_665 2_765
C17 Ag2 Ag1 90.7(3) . .
C25 Ag2 Ag1 88.6(3) . .
Ag3 Ag2 Ag1 124.92(3) 2_765 .
Ag5 Ag2 Ag1 125.0(2) 2_765 .
Ag5 Ag2 Ag1 58.83(15) . .
Ag3 Ag2 Ag1 59.22(3) . .
Ag4 Ag2 Ag1 57.84(3) 2_665 .
Ag5' Ag2 Ag1 118.8(4) 2_765 .
C17 Ag2 Ag5' 54.0(5) . .
C25 Ag2 Ag5' 132.5(5) . .
Ag3 Ag2 Ag5' 60.3(4) 2_765 .
Ag5 Ag2 Ag5' 110.7(3) 2_765 .
Ag5 Ag2 Ag5' 6.7(4) . .
Ag3 Ag2 Ag5' 80.7(4) . .
Ag4 Ag2 Ag5' 79.67(11) 2_665 .
Ag5' Ag2 Ag5' 111.62(17) 2_765 .
Ag1 Ag2 Ag5' 64.6(4) . .
O2 Ag3 C9 111.4(4) . .
O2 Ag3 C25 104.5(4) . .
C9 Ag3 C25 124.0(3) . .
O2 Ag3 C17 99.1(4) . 2_765
C9 Ag3 C17 115.7(3) . 2_765
C25 Ag3 C17 98.6(4) . 2_765
O2 Ag3 C10 95.2(4) . .
C9 Ag3 C10 27.1(3) . .
C25 Ag3 C10 151.1(3) . .
C17 Ag3 C10 99.0(3) 2_765 .
O2 Ag3 Ag5' 111.2(5) . 2_765
C9 Ag3 Ag5' 137.2(4) . 2_765
C25 Ag3 Ag5' 46.2(3) . 2_765
C17 Ag3 Ag5' 52.5(3) 2_765 2_765
C10 Ag3 Ag5' 142.7(4) . 2_765
O2 Ag3 Ag2 139.7(3) . 2_765
C9 Ag3 Ag2 82.9(3) . 2_765
C25 Ag3 Ag2 96.4(3) . 2_765
C17 Ag3 Ag2 43.1(2) 2_765 2_765
C10 Ag3 Ag2 81.2(2) . 2_765
Ag5' Ag3 Ag2 61.6(3) 2_765 2_765
O2 Ag3 Ag2 144.9(3) . .
C9 Ag3 Ag2 87.0(2) . .
C25 Ag3 Ag2 43.0(3) . .
C17 Ag3 Ag2 99.0(2) 2_765 .
C10 Ag3 Ag2 111.3(2) . .
Ag5' Ag3 Ag2 59.7(3) 2_765 .
Ag2 Ag3 Ag2 69.59(3) 2_765 .
O2 Ag3 Ag1 111.8(3) . .
C9 Ag3 Ag1 42.4(2) . .
C25 Ag3 Ag1 85.1(3) . .
C17 Ag3 Ag1 146.9(2) 2_765 .
C10 Ag3 Ag1 67.8(2) . .
Ag5' Ag3 Ag1 121.1(2) 2_765 .
Ag2 Ag3 Ag1 103.87(3) 2_765 .
Ag2 Ag3 Ag1 61.84(3) . .
O2 Ag3 Ag5 116.1(3) . 2_765
C9 Ag3 Ag5 132.3(3) . 2_765
C25 Ag3 Ag5 46.8(3) . 2_765
C17 Ag3 Ag5 52.7(3) 2_765 2_765
C10 Ag3 Ag5 139.1(3) . 2_765
Ag5' Ag3 Ag5 4.9(4) 2_765 2_765
Ag2 Ag3 Ag5 57.92(14) 2_765 2_765
Ag2 Ag3 Ag5 56.1(2) . 2_765
Ag1 Ag3 Ag5 117.9(2) . 2_765
O1 Ag4 C1 108.6(4) . .
O1 Ag4 C17 98.5(4) . 2_665
C1 Ag4 C17 127.0(3) . 2_665
O1 Ag4 C18 90.5(4) . 2_665
C1 Ag4 C18 152.2(4) . 2_665
C17 Ag4 C18 26.7(3) 2_665 2_665
O1 Ag4 C9 112.2(3) . .
C1 Ag4 C9 96.8(3) . .
C17 Ag4 C9 114.0(3) 2_665 .
C18 Ag4 C9 94.2(4) 2_665 .
O1 Ag4 Ag1 149.4(2) . .
C1 Ag4 Ag1 94.5(3) . .
C17 Ag4 Ag1 82.3(3) 2_665 .
C18 Ag4 Ag1 76.4(3) 2_665 .
C9 Ag4 Ag1 43.2(2) . .
O1 Ag4 Ag1 138.6(2) . 2_665
C1 Ag4 Ag1 43.7(3) . 2_665
C17 Ag4 Ag1 86.5(2) 2_665 2_665
C18 Ag4 Ag1 108.8(3) 2_665 2_665
C9 Ag4 Ag1 102.7(2) . 2_665
Ag1 Ag4 Ag1 71.95(3) . 2_665
O1 Ag4 Ag2 94.8(3) . 2_665
C1 Ag4 Ag2 90.1(2) . 2_665
C17 Ag4 Ag2 41.9(2) 2_665 2_665
C18 Ag4 Ag2 67.7(3) 2_665 2_665
C9 Ag4 Ag2 148.0(2) . 2_665
Ag1 Ag4 Ag2 105.25(3) . 2_665
Ag1 Ag4 Ag2 62.23(3) 2_665 2_665
O1 Ag4 Ag5 125.1(4) . .
C1 Ag4 Ag5 47.0(3) . .
C17 Ag4 Ag5 136.3(3) 2_665 .
C18 Ag4 Ag5 135.0(3) 2_665 .
C9 Ag4 Ag5 50.0(3) . .
Ag1 Ag4 Ag5 58.88(15) . .
Ag1 Ag4 Ag5 64.2(2) 2_665 .
Ag2 Ag4 Ag5 126.4(2) 2_665 .
Ag5' Ag5 C1 86(2) . .
Ag5' Ag5 C25 56(2) . 2_765
C1 Ag5 C25 119.5(5) . 2_765
Ag5' Ag5 C9 175(3) . .
C1 Ag5 C9 98.7(5) . .
C25 Ag5 C9 118.7(6) 2_765 .
Ag5' Ag5 C17 60(3) . .
C1 Ag5 C17 105.0(5) . .
C25 Ag5 C17 95.0(5) 2_765 .
C9 Ag5 C17 120.6(5) . .
Ag5' Ag5 Ag2 94(3) . 2_765
C1 Ag5 Ag2 153.9(5) . 2_765
C25 Ag5 Ag2 43.9(3) 2_765 2_765
C9 Ag5 Ag2 80.7(4) . 2_765
C17 Ag5 Ag2 97.4(4) . 2_765
Ag5' Ag5 Ag2 93(3) . .
C1 Ag5 Ag2 136.5(5) . .
C25 Ag5 Ag2 94.8(4) 2_765 .
C9 Ag5 Ag2 85.3(3) . .
C17 Ag5 Ag2 41.7(3) . .
Ag2 Ag5 Ag2 69.5(2) 2_765 .
Ag5' Ag5 Ag1 141(3) . .
C1 Ag5 Ag1 92.1(4) . .
C25 Ag5 Ag1 147.5(5) 2_765 .
C9 Ag5 Ag1 42.4(2) . .
C17 Ag5 Ag1 82.7(4) . .
Ag2 Ag5 Ag1 104.0(2) 2_765 .
Ag2 Ag5 Ag1 62.23(17) . .
Ag5' Ag5 Ag3 46(2) . 2_765
C1 Ag5 Ag3 131.0(4) . 2_765
C25 Ag5 Ag3 47.0(3) 2_765 2_765
C9 Ag5 Ag3 129.9(4) . 2_765
C17 Ag5 Ag3 48.8(3) . 2_765
Ag2 Ag5 Ag3 58.02(18) 2_765 2_765
Ag2 Ag5 Ag3 55.88(19) . 2_765
Ag1 Ag5 Ag3 118.0(3) . 2_765
Ag5' Ag5 Ag4 133(3) . .
C1 Ag5 Ag4 46.8(3) . .
C25 Ag5 Ag4 141.9(5) 2_765 .
C9 Ag5 Ag4 52.1(3) . .
C17 Ag5 Ag4 122.1(4) . .
Ag2 Ag5 Ag4 128.6(3) 2_765 .
Ag2 Ag5 Ag4 118.3(2) . .
Ag1 Ag5 Ag4 56.25(14) . .
Ag3 Ag5 Ag4 170.9(4) 2_765 .
Ag5' Ag5 Ag1 89(3) . 2_665
C1 Ag5 Ag1 38.8(3) . 2_665
C25 Ag5 Ag1 143.4(4) 2_765 2_665
C9 Ag5 Ag1 96.5(3) . 2_665
C17 Ag5 Ag1 73.0(4) . 2_665
Ag2 Ag5 Ag1 167.1(4) 2_765 2_665
Ag2 Ag5 Ag1 97.8(3) . 2_665
Ag1 Ag5 Ag1 66.8(2) . 2_665
Ag3 Ag5 Ag1 117.2(3) 2_765 2_665
Ag4 Ag5 Ag1 54.87(17) . 2_665
Ag5 Ag5' C25 116(3) . 2_765
Ag5 Ag5' C1 85(3) . .
C25 Ag5' C1 127.7(6) 2_765 .
Ag5 Ag5' C17 113(3) . .
C25 Ag5' C17 104.4(7) 2_765 .
C1 Ag5' C17 110.2(5) . .
Ag5 Ag5' C26 131(3) . 2_765
C25 Ag5' C26 25.7(6) 2_765 2_765
C1 Ag5' C26 104.2(7) . 2_765
C17 Ag5' C26 108.7(9) . 2_765
Ag5 Ag5' C2 89(3) . .
C25 Ag5' C2 102.9(5) 2_765 .
C1 Ag5' C2 26.2(3) . .
C17 Ag5' C2 131.9(6) . .
C26 Ag5' C2 82.1(6) 2_765 .
Ag5 Ag5' Ag3 129(3) . 2_765
C25 Ag5' Ag3 51.6(4) 2_765 2_765
C1 Ag5' Ag3 144.4(9) . 2_765
C17 Ag5' Ag3 53.0(4) . 2_765
C26 Ag5' Ag3 62.6(6) 2_765 2_765
C2 Ag5' Ag3 139.0(8) . 2_765
Ag5 Ag5' Ag2 79(3) . 2_765
C25 Ag5' Ag2 43.4(3) 2_765 2_765
C1 Ag5' Ag2 149.7(6) . 2_765
C17 Ag5' Ag2 99.8(3) . 2_765
C26 Ag5' Ag2 68.8(5) 2_765 2_765
C2 Ag5' Ag2 126.9(4) . 2_765
Ag3 Ag5' Ag2 60.28(15) 2_765 2_765
Ag5 Ag5' Ag2 80(3) . .
C25 Ag5' Ag2 97.5(3) 2_765 .
C1 Ag5' Ag2 134.2(5) . .
C17 Ag5' Ag2 41.7(3) . .
C26 Ag5' Ag2 118.1(6) 2_765 .
C2 Ag5' Ag2 159.5(6) . .
Ag3 Ag5' Ag2 58.02(14) 2_765 .
Ag2 Ag5' Ag2 68.38(17) 2_765 .
Ag5 Ag5' Ag1 85(3) . 2_665
C25 Ag5' Ag1 156.4(9) 2_765 2_665
C1 Ag5' Ag1 38.6(3) . 2_665
C17 Ag5' Ag1 74.7(3) . 2_665
C26 Ag5' Ag1 131.4(8) 2_765 2_665
C2 Ag5' Ag1 64.7(3) . 2_665
Ag3 Ag5' Ag1 124.2(4) 2_765 2_665
Ag2 Ag5' Ag1 159.9(7) 2_765 2_665
Ag2 Ag5' Ag1 96.7(2) . 2_665
C2 C1 Ag1 169.9(10) . 2_665
C2 C1 Ag4 99.9(9) . .
Ag1 C1 Ag4 85.2(4) 2_665 .
C2 C1 Ag5' 91.7(8) . .
Ag1 C1 Ag5' 96.5(4) 2_665 .
Ag4 C1 Ag5' 95.0(7) . .
C2 C1 Ag5 92.9(9) . .
Ag1 C1 Ag5 96.2(5) 2_665 .
Ag4 C1 Ag5 86.2(4) . .
Ag5' C1 Ag5 8.8(5) . .
C1 C2 C3 175.5(13) . .
C1 C2 Ag5' 62.0(7) . .
C3 C2 Ag5' 122.3(7) . .
C4 C3 C8 120.0 . .
C4 C3 C2 119.0(8) . .
C8 C3 C2 120.8(8) . .
C3 C4 C5 120.0 . .
C3 C4 H4 120.0 . .
C5 C4 H4 120.0 . .
C6 C5 C4 120.0 . .
C6 C5 H5 120.0 . .
C4 C5 H5 120.0 . .
C5 C6 C7 120.0 . .
C5 C6 H6 120.0 . .
C7 C6 H6 120.0 . .
C6 C7 C8 120.0 . .
C6 C7 H7 120.0 . .
C8 C7 H7 120.0 . .
C7 C8 C3 120.0 . .
C7 C8 H8 120.0 . .
C3 C8 H8 120.0 . .
C10 C9 Ag1 155.3(9) . .
C10 C9 Ag3 89.3(7) . .
Ag1 C9 Ag3 86.1(4) . .
C10 C9 Ag5 122.3(9) . .
Ag1 C9 Ag5 82.4(4) . .
Ag3 C9 Ag5 97.7(4) . .
C10 C9 Ag4 106.5(8) . .
Ag1 C9 Ag4 77.7(3) . .
Ag3 C9 Ag4 163.6(4) . .
Ag5 C9 Ag4 77.9(4) . .
C9 C10 C11 174.0(11) . .
C9 C10 Ag3 63.6(7) . .
C11 C10 Ag3 121.9(7) . .
C12 C11 C16 120.0 . .
C12 C11 C10 120.6(7) . .
C16 C11 C10 119.3(7) . .
C13 C12 C11 120.0 . .
C13 C12 H12 120.0 . .
C11 C12 H12 120.0 . .
C12 C13 C14 120.0 . .
C12 C13 H13 120.0 . .
C14 C13 H13 120.0 . .
C15 C14 C13 120.0 . .
C15 C14 H14 120.0 . .
C13 C14 H14 120.0 . .
C16 C15 C14 120.0 . .
C16 C15 H15 120.0 . .
C14 C15 H15 120.0 . .
C15 C16 C11 120.0 . .
C15 C16 H16 120.0 . .
C11 C16 H16 120.0 . .
C18 C17 Ag2 157.2(10) . .
C18 C17 Ag5' 116.7(10) . .
Ag2 C17 Ag5' 84.3(5) . .
C18 C17 Ag4 81.6(8) . 2_665
Ag2 C17 Ag4 84.6(4) . 2_665
Ag5' C17 Ag4 104.5(5) . 2_665
C18 C17 Ag3 112.7(9) . 2_765
Ag2 C17 Ag3 80.1(3) . 2_765
Ag5' C17 Ag3 74.5(4) . 2_765
Ag4 C17 Ag3 164.7(5) 2_665 2_765
C18 C17 Ag5 121.1(9) . .
Ag2 C17 Ag5 79.0(4) . .
Ag5' C17 Ag5 7.2(5) . .
Ag4 C17 Ag5 99.1(4) 2_665 .
Ag3 C17 Ag5 78.5(4) 2_765 .
C17 C18 C19 174.7(11) . .
C17 C18 Ag4 71.7(8) . 2_665
C19 C18 Ag4 113.0(8) . 2_665
C20 C19 C24 120.0 . .
C20 C19 C18 118.7(8) . .
C24 C19 C18 121.3(8) . .
C19 C20 C21 120.0 . .
C19 C20 H20 120.0 . .
C21 C20 H20 120.0 . .
C22 C21 C20 120.0 . .
C22 C21 H21 120.0 . .
C20 C21 H21 120.0 . .
C23 C22 C21 120.0 . .
C23 C22 H22 120.0 . .
C21 C22 H22 120.0 . .
C24 C23 C22 120.0 . .
C24 C23 H23 120.0 . .
C22 C23 H23 120.0 . .
C23 C24 C19 120.0 . .
C23 C24 H24 120.0 . .
C19 C24 H24 120.0 . .
C26 C25 C26' 40.4(13) . .
C26 C25 Ag2 164.2(13) . .
C26' C25 Ag2 130.7(14) . .
C26 C25 Ag5' 100.5(13) . 2_765
C26' C25 Ag5' 139.7(16) . 2_765
Ag2 C25 Ag5' 89.6(6) . 2_765
C26 C25 Ag5 105.7(13) . 2_765
C26' C25 Ag5 145.8(15) . 2_765
Ag2 C25 Ag5 83.2(4) . 2_765
Ag5' C25 Ag5 7.8(6) 2_765 2_765
C26 C25 Ag3 108.0(13) . .
C26' C25 Ag3 99.1(13) . .
Ag2 C25 Ag3 85.2(4) . .
Ag5' C25 Ag3 82.2(5) 2_765 .
Ag5 C25 Ag3 86.2(5) 2_765 .
C25 C26 C27 172(2) . .
C25 C26 Ag5' 53.7(11) . 2_765
C27 C26 Ag5' 133.7(15) . 2_765
C28 C27 C32 120.0 . .
C28 C27 C26 122.7(14) . .
C32 C27 C26 117.2(15) . .
C27 C28 C29 120.0 . .
C28 C29 C30 120.0 . .
C28 C29 C30 136.0(19) . 2_764
C30 C29 C30 35(2) . 2_764
C30 C30 C31 116(4) 2_764 .
C30 C30 C29 101(4) 2_764 .
C31 C30 C29 120.0 . .
C30 C30 C29 44.0(17) 2_764 2_764
C31 C30 C29 84(3) . 2_764
C29 C30 C29 145(3) . 2_764
C32 C31 C30 120.0 . .
C32 C31 H31 120.0 . .
C30 C31 H31 120.0 . .
C31 C32 C27 120.0 . .
C31 C32 H32 120.0 . .
C27 C32 H32 120.0 . .
C25 C26' C27' 174(2) . .
C28' C27' C32' 120.0 . .
C28' C27' C26' 115.3(14) . .
C32' C27' C26' 124.6(14) . .
C27' C28' C29' 120.0 . .
C30' C29' C28' 120.0 . .
C31' C30' C29' 120.0 . .
C31' C30' C30' 143(3) . 2_664
C29' C30' C30' 95(3) . 2_664
C30' C31' C32' 120.0 . .
C30' C31' H31' 120.0 . .
C32' C31' H31' 120.0 . .
C31' C32' C27' 120.0 . .
C31' C32' H32' 120.0 . .
C27' C32' H32' 120.0 . .
S1' O1 S1 39.1(8) . .
S1' O1 Ag4 131.5(13) . .
S1 O1 Ag4 127.3(6) . .
O1 S1 C34 107.9(13) . .
O1 S1 C33 104.6(11) . .
C34 S1 C33 92(2) . .
S2 O2 S2' 83.1(12) . .
S2 O2 Ag3 150.5(11) . .
S2' O2 Ag3 124.4(9) . .
O2 S2 C35 118.2(19) . .
O2 S2 C36 109(2) . .
C35 S2 C36 76(3) . .
F6 Sb1 F4 91.6(12) . .
F6 Sb1 F5 98.6(15) . .
F4 Sb1 F5 87.3(15) . .
F6 Sb1 F1 87.9(13) . .
F4 Sb1 F1 178.3(13) . .
F5 Sb1 F1 94.4(14) . .
F6 Sb1 F3 178.1(9) . .
F4 Sb1 F3 89.7(10) . .
F5 Sb1 F3 82.8(12) . .
F1 Sb1 F3 90.7(11) . .
F6 Sb1 F2 90.7(14) . .
F4 Sb1 F2 95.9(13) . .
F5 Sb1 F2 170.1(11) . .
F1 Sb1 F2 82.5(10) . .
F3 Sb1 F2 87.9(9) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ag1 C9 2.072(10) .
Ag1 C1 2.090(10) 2_665
Ag1 Ag4 2.9580(12) .
Ag1 Ag4 3.0132(12) 2_665
Ag1 Ag3 3.0686(12) .
Ag1 Ag5 3.045(7) .
Ag1 Ag2 3.1492(12) .
Ag1 Ag5 3.317(11) 2_665
Ag1 Ag5' 3.328(6) 2_665
Ag2 C17 2.066(11) .
Ag2 C25 2.092(11) .
Ag2 Ag3 2.9786(13) 2_765
Ag2 Ag5 2.995(11) 2_765
Ag2 Ag5 3.049(10) .
Ag2 Ag3 3.0598(13) .
Ag2 Ag4 3.0803(12) 2_665
Ag2 Ag5' 3.042(7) 2_765
Ag2 Ag5' 3.090(7) .
Ag3 O2 2.278(10) .
Ag3 C9 2.409(10) .
Ag3 C25 2.413(11) .
Ag3 C17 2.528(10) 2_765
Ag3 C10 2.690(11) .
Ag3 Ag5' 3.051(15) 2_765
Ag3 Ag2 2.9786(13) 2_765
Ag3 Ag5 3.292(10) 2_765
Ag4 O1 2.322(9) .
Ag4 C1 2.352(10) .
Ag4 C17 2.487(10) 2_665
Ag4 C18 2.592(12) 2_665
Ag4 C9 2.598(10) .
Ag4 Ag1 3.0132(12) 2_665
Ag4 Ag2 3.0803(12) 2_665
Ag4 Ag5 3.221(10) .
Ag5 Ag5' 0.36(2) .
Ag5 C1 2.361(14) .
Ag5 C25 2.404(15) 2_765
Ag5 C9 2.521(13) .
Ag5 C17 2.672(16) .
Ag5 Ag2 2.995(11) 2_765
Ag5 Ag3 3.292(10) 2_765
Ag5 Ag1 3.317(11) 2_665
Ag5' C25 2.224(16) 2_765
Ag5' C1 2.363(12) .
Ag5' C17 2.511(14) .
Ag5' C26 2.71(3) 2_765
Ag5' C2 2.674(13) .
Ag5' Ag3 3.052(15) 2_765
Ag5' Ag2 3.042(7) 2_765
Ag5' Ag1 3.328(6) 2_665
C1 C2 1.183(14) .
C1 Ag1 2.090(10) 2_665
C2 C3 1.445(12) .
C3 C4 1.3900 .
C3 C8 1.3900 .
C4 C5 1.3900 .
C4 H4 0.9300 .
C5 C6 1.3900 .
C5 H5 0.9300 .
C6 C7 1.3900 .
C6 H6 0.9300 .
C7 C8 1.3900 .
C7 H7 0.9300 .
C8 H8 0.9300 .
C9 C10 1.227(14) .
C10 C11 1.439(12) .
C11 C12 1.3900 .
C11 C16 1.3900 .
C12 C13 1.3900 .
C12 H12 0.9300 .
C13 C14 1.3900 .
C13 H13 0.9300 .
C14 C15 1.3900 .
C14 H14 0.9300 .
C15 C16 1.3900 .
C15 H15 0.9300 .
C16 H16 0.9300 .
C17 C18 1.179(15) .
C17 Ag4 2.487(10) 2_665
C17 Ag3 2.528(10) 2_765
C18 C19 1.474(15) .
C18 Ag4 2.592(12) 2_665
C19 C20 1.3900 .
C19 C24 1.3900 .
C20 C21 1.3900 .
C20 H20 0.9300 .
C21 C22 1.3900 .
C21 H21 0.9300 .
C22 C23 1.3900 .
C22 H22 0.9300 .
C23 C24 1.3900 .
C23 H23 0.9300 .
C24 H24 0.9300 .
C25 C26 1.20(3) .
C25 C26' 1.212(10) .
C25 Ag5' 2.224(16) 2_765
C25 Ag5 2.404(14) 2_765
C26 C27 1.40(3) .
C26 Ag5' 2.71(3) 2_765
C27 C28 1.3900 .
C27 C32 1.3900 .
C28 C29 1.3900 .
C29 C30 1.3900 .
C29 C30 1.96(5) 2_764
C30 C30 1.14(4) 2_764
C30 C31 1.3900 .
C30 C29 1.96(4) 2_764
C31 C32 1.3900 .
C31 H31 0.9300 .
C32 H32 0.9300 .
C26' C27' 1.529(18) .
C27' C28' 1.3900 .
C27' C32' 1.3900 .
C28' C29' 1.3900 .
C29' C30' 1.3900 .
C30' C31' 1.3900 .
C30' C30' 1.72(3) 2_664
C31' C32' 1.3900 .
C31' H31' 0.9300 .
C32' H32' 0.9300 .
O1 S1' 1.452(19) .
O1 S1 1.490(11) .
S1 C34 1.727(10) .
S1 C33 1.75(3) .
O2 S2 1.463(9) .
O2 S2' 1.488(17) .
S2 C35 1.728(10) .
S2 C36 1.724(10) .
Sb1 F6 1.709(18) .
Sb1 F4 1.732(14) .
Sb1 F5 1.76(2) .
Sb1 F1 1.796(15) .
Sb1 F3 1.820(15) .
Sb1 F2 1.875(15) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
C9 Ag1 Ag2 C17 100.4(4) . .
C1 Ag1 Ag2 C17 -85.2(4) 2_665 .
Ag4 Ag1 Ag2 C17 47.8(3) . .
Ag4 Ag1 Ag2 C17 -44.8(3) 2_665 .
Ag3 Ag1 Ag2 C17 143.2(3) . .
Ag5 Ag1 Ag2 C17 52.9(4) . .
Ag5 Ag1 Ag2 C17 -47.3(3) 2_665 .
Ag5' Ag1 Ag2 C17 -51.7(4) 2_665 .
C9 Ag1 Ag2 C25 -87.9(4) . .
C1 Ag1 Ag2 C25 86.5(4) 2_665 .
Ag4 Ag1 Ag2 C25 -140.5(3) . .
Ag4 Ag1 Ag2 C25 126.9(3) 2_665 .
Ag3 Ag1 Ag2 C25 -45.1(3) . .
Ag5 Ag1 Ag2 C25 -135.4(4) . .
Ag5 Ag1 Ag2 C25 124.4(3) 2_665 .
Ag5' Ag1 Ag2 C25 120.0(4) 2_665 .
C9 Ag1 Ag2 Ag3 51.8(3) . 2_765
C1 Ag1 Ag2 Ag3 -133.8(3) 2_665 2_765
Ag4 Ag1 Ag2 Ag3 -0.84(6) . 2_765
Ag4 Ag1 Ag2 Ag3 -93.42(4) 2_665 2_765
Ag3 Ag1 Ag2 Ag3 94.54(4) . 2_765
Ag5 Ag1 Ag2 Ag3 4.3(3) . 2_765
Ag5 Ag1 Ag2 Ag3 -95.92(16) 2_665 2_765
Ag5' Ag1 Ag2 Ag3 -100.3(3) 2_665 2_765
C9 Ag1 Ag2 Ag5 -46.8(4) . 2_765
C1 Ag1 Ag2 Ag5 127.6(4) 2_665 2_765
Ag4 Ag1 Ag2 Ag5 -99.4(2) . 2_765
Ag4 Ag1 Ag2 Ag5 168.0(2) 2_665 2_765
Ag3 Ag1 Ag2 Ag5 -4.1(2) . 2_765
Ag5 Ag1 Ag2 Ag5 -94.3(3) . 2_765
Ag5 Ag1 Ag2 Ag5 165.5(4) 2_665 2_765
Ag5' Ag1 Ag2 Ag5 161.1(4) 2_665 2_765
C9 Ag1 Ag2 Ag5 47.5(4) . .
C1 Ag1 Ag2 Ag5 -138.1(4) 2_665 .
Ag4 Ag1 Ag2 Ag5 -5.1(3) . .
Ag4 Ag1 Ag2 Ag5 -97.7(3) 2_665 .
Ag3 Ag1 Ag2 Ag5 90.3(3) . .
Ag5 Ag1 Ag2 Ag5 -100.2(3) 2_665 .
Ag5' Ag1 Ag2 Ag5 -104.6(4) 2_665 .
C9 Ag1 Ag2 Ag3 -42.8(3) . .
C1 Ag1 Ag2 Ag3 131.6(3) 2_665 .
Ag4 Ag1 Ag2 Ag3 -95.38(4) . .
Ag4 Ag1 Ag2 Ag3 172.05(4) 2_665 .
Ag5 Ag1 Ag2 Ag3 -90.3(3) . .
Ag5 Ag1 Ag2 Ag3 169.54(16) 2_665 .
Ag5' Ag1 Ag2 Ag3 165.1(3) 2_665 .
C9 Ag1 Ag2 Ag4 145.2(3) . 2_665
C1 Ag1 Ag2 Ag4 -40.4(3) 2_665 2_665
Ag4 Ag1 Ag2 Ag4 92.58(4) . 2_665
Ag3 Ag1 Ag2 Ag4 -172.05(4) . 2_665
Ag5 Ag1 Ag2 Ag4 97.7(3) . 2_665
Ag5 Ag1 Ag2 Ag4 -2.51(16) 2_665 2_665
Ag5' Ag1 Ag2 Ag4 -6.9(3) 2_665 2_665
C9 Ag1 Ag2 Ag5' -50.3(4) . 2_765
C1 Ag1 Ag2 Ag5' 124.1(4) 2_665 2_765
Ag4 Ag1 Ag2 Ag5' -102.9(2) . 2_765
Ag4 Ag1 Ag2 Ag5' 164.5(2) 2_665 2_765
Ag3 Ag1 Ag2 Ag5' -7.5(2) . 2_765
Ag5 Ag1 Ag2 Ag5' -97.8(4) . 2_765
Ag5 Ag1 Ag2 Ag5' 162.0(3) 2_665 2_765
Ag5' Ag1 Ag2 Ag5' 157.6(6) 2_665 2_765
C9 Ag1 Ag2 Ag5' 51.5(4) . .
C1 Ag1 Ag2 Ag5' -134.1(4) 2_665 .
Ag4 Ag1 Ag2 Ag5' -1.1(3) . .
Ag4 Ag1 Ag2 Ag5' -93.7(3) 2_665 .
Ag3 Ag1 Ag2 Ag5' 94.3(3) . .
Ag5 Ag1 Ag2 Ag5' 4.0(4) . .
Ag5 Ag1 Ag2 Ag5' -96.2(3) 2_665 .
Ag5' Ag1 Ag2 Ag5' -100.61(17) 2_665 .
C17 Ag2 Ag3 O2 -144.7(7) . .
C25 Ag2 Ag3 O2 27.3(7) . .
Ag3 Ag2 Ag3 O2 152.3(6) 2_765 .
Ag5 Ag2 Ag3 O2 88.0(6) 2_765 .
Ag5 Ag2 Ag3 O2 -150.8(6) . .
Ag4 Ag2 Ag3 O2 -80.9(6) 2_665 .
Ag5' Ag2 Ag3 O2 84.0(6) 2_765 .
Ag1 Ag2 Ag3 O2 -88.4(5) . .
Ag5' Ag2 Ag3 O2 -154.3(6) . .
C17 Ag2 Ag3 C9 -20.5(5) . .
C25 Ag2 Ag3 C9 151.4(5) . .
Ag3 Ag2 Ag3 C9 -83.5(2) 2_765 .
Ag5 Ag2 Ag3 C9 -147.9(3) 2_765 .
Ag5 Ag2 Ag3 C9 -26.7(3) . .
Ag4 Ag2 Ag3 C9 43.3(2) 2_665 .
Ag5' Ag2 Ag3 C9 -151.8(4) 2_765 .
Ag1 Ag2 Ag3 C9 35.8(2) . .
Ag5' Ag2 Ag3 C9 -30.1(3) . .
C17 Ag2 Ag3 C25 -171.9(6) . .
Ag3 Ag2 Ag3 C25 125.1(4) 2_765 .
Ag5 Ag2 Ag3 C25 60.7(4) 2_765 .
Ag5 Ag2 Ag3 C25 -178.1(4) . .
Ag4 Ag2 Ag3 C25 -108.1(4) 2_665 .
Ag5' Ag2 Ag3 C25 56.7(5) 2_765 .
Ag1 Ag2 Ag3 C25 -115.7(4) . .
Ag5' Ag2 Ag3 C25 178.5(5) . .
C17 Ag2 Ag3 C17 95.1(4) . 2_765
C25 Ag2 Ag3 C17 -93.0(5) . 2_765
Ag3 Ag2 Ag3 C17 32.1(3) 2_765 2_765
Ag5 Ag2 Ag3 C17 -32.3(3) 2_765 2_765
Ag5 Ag2 Ag3 C17 88.9(3) . 2_765
Ag4 Ag2 Ag3 C17 158.9(3) 2_665 2_765
Ag5' Ag2 Ag3 C17 -36.2(4) 2_765 2_765
Ag1 Ag2 Ag3 C17 151.4(3) . 2_765
Ag5' Ag2 Ag3 C17 85.5(3) . 2_765
C17 Ag2 Ag3 C10 -8.3(5) . .
C25 Ag2 Ag3 C10 163.7(5) . .
Ag3 Ag2 Ag3 C10 -71.3(2) 2_765 .
Ag5 Ag2 Ag3 C10 -135.6(3) 2_765 .
Ag5 Ag2 Ag3 C10 -14.4(3) . .
Ag4 Ag2 Ag3 C10 55.5(2) 2_665 .
Ag5' Ag2 Ag3 C10 -139.6(4) 2_765 .
Ag1 Ag2 Ag3 C10 48.0(2) . .
Ag5' Ag2 Ag3 C10 -17.9(3) . .
C17 Ag2 Ag3 Ag5' 131.3(5) . 2_765
C25 Ag2 Ag3 Ag5' -56.7(5) . 2_765
Ag3 Ag2 Ag3 Ag5' 68.3(3) 2_765 2_765
Ag5 Ag2 Ag3 Ag5' 4.0(4) 2_765 2_765
Ag5 Ag2 Ag3 Ag5' 125.2(3) . 2_765
Ag4 Ag2 Ag3 Ag5' -164.9(3) 2_665 2_765
Ag1 Ag2 Ag3 Ag5' -172.4(3) . 2_765
Ag5' Ag2 Ag3 Ag5' 121.72(13) . 2_765
C17 Ag2 Ag3 Ag2 63.0(4) . 2_765
C25 Ag2 Ag3 Ag2 -125.1(4) . 2_765
Ag3 Ag2 Ag3 Ag2 0.0 2_765 2_765
Ag5 Ag2 Ag3 Ag2 -64.36(18) 2_765 2_765
Ag5 Ag2 Ag3 Ag2 56.86(19) . 2_765
Ag4 Ag2 Ag3 Ag2 126.82(5) 2_665 2_765
Ag5' Ag2 Ag3 Ag2 -68.3(3) 2_765 2_765
Ag1 Ag2 Ag3 Ag2 119.29(4) . 2_765
Ag5' Ag2 Ag3 Ag2 53.4(2) . 2_765
C17 Ag2 Ag3 Ag1 -56.3(4) . .
C25 Ag2 Ag3 Ag1 115.7(4) . .
Ag3 Ag2 Ag3 Ag1 -119.29(4) 2_765 .
Ag5 Ag2 Ag3 Ag1 176.36(18) 2_765 .
Ag5 Ag2 Ag3 Ag1 -62.43(18) . .
Ag4 Ag2 Ag3 Ag1 7.53(3) 2_665 .
Ag5' Ag2 Ag3 Ag1 172.4(3) 2_765 .
Ag5' Ag2 Ag3 Ag1 -65.9(2) . .
C17 Ag2 Ag3 Ag5 127.4(4) . 2_765
C25 Ag2 Ag3 Ag5 -60.7(4) . 2_765
Ag3 Ag2 Ag3 Ag5 64.36(18) 2_765 2_765
Ag5 Ag2 Ag3 Ag5 121.2(2) . 2_765
Ag4 Ag2 Ag3 Ag5 -168.83(18) 2_665 2_765
Ag5' Ag2 Ag3 Ag5 -4.0(4) 2_765 2_765
Ag1 Ag2 Ag3 Ag5 -176.36(18) . 2_765
Ag5' Ag2 Ag3 Ag5 117.8(3) . 2_765
C9 Ag1 Ag3 O2 -98.3(5) . .
C1 Ag1 Ag3 O2 73.1(5) 2_665 .
Ag4 Ag1 Ag3 O2 -100.6(3) . .
Ag4 Ag1 Ag3 O2 133.9(3) 2_665 .
Ag5 Ag1 Ag3 O2 -155.6(4) . .
Ag2 Ag1 Ag3 O2 141.8(3) . .
Ag5 Ag1 Ag3 O2 50.6(12) 2_665 .
Ag5' Ag1 Ag3 O2 26.5(11) 2_665 .
C1 Ag1 Ag3 C9 171.4(5) 2_665 .
Ag4 Ag1 Ag3 C9 -2.3(4) . .
Ag4 Ag1 Ag3 C9 -127.7(4) 2_665 .
Ag5 Ag1 Ag3 C9 -57.3(4) . .
Ag2 Ag1 Ag3 C9 -119.9(4) . .
Ag5 Ag1 Ag3 C9 148.9(12) 2_665 .
Ag5' Ag1 Ag3 C9 124.8(11) 2_665 .
C9 Ag1 Ag3 C25 158.0(5) . .
C1 Ag1 Ag3 C25 -30.6(5) 2_665 .
Ag4 Ag1 Ag3 C25 155.7(3) . .
Ag4 Ag1 Ag3 C25 30.2(3) 2_665 .
Ag5 Ag1 Ag3 C25 100.7(4) . .
Ag2 Ag1 Ag3 C25 38.1(3) . .
Ag5 Ag1 Ag3 C25 -53.2(12) 2_665 .
Ag5' Ag1 Ag3 C25 -77.2(11) 2_665 .
C9 Ag1 Ag3 C17 59.7(6) . 2_765
C1 Ag1 Ag3 C17 -128.8(6) 2_665 2_765
Ag4 Ag1 Ag3 C17 57.5(5) . 2_765
Ag4 Ag1 Ag3 C17 -68.0(5) 2_665 2_765
Ag5 Ag1 Ag3 C17 2.4(5) . 2_765
Ag2 Ag1 Ag3 C17 -60.2(4) . 2_765
Ag5 Ag1 Ag3 C17 -151.4(12) 2_665 2_765
Ag5' Ag1 Ag3 C17 -175.5(11) 2_665 2_765
C9 Ag1 Ag3 C10 -11.7(5) . .
C1 Ag1 Ag3 C10 159.8(4) 2_665 .
Ag4 Ag1 Ag3 C10 -14.0(2) . .
Ag4 Ag1 Ag3 C10 -139.4(3) 2_665 .
Ag5 Ag1 Ag3 C10 -69.0(3) . .
Ag2 Ag1 Ag3 C10 -131.6(2) . .
Ag5 Ag1 Ag3 C10 137.2(12) 2_665 .
Ag5' Ag1 Ag3 C10 113.1(11) 2_665 .
C9 Ag1 Ag3 Ag5' 127.6(5) . 2_765
C1 Ag1 Ag3 Ag5' -61.0(5) 2_665 2_765
Ag4 Ag1 Ag3 Ag5' 125.3(3) . 2_765
Ag4 Ag1 Ag3 Ag5' -0.2(3) 2_665 2_765
Ag5 Ag1 Ag3 Ag5' 70.3(3) . 2_765
Ag2 Ag1 Ag3 Ag5' 7.7(3) . 2_765
Ag5 Ag1 Ag3 Ag5' -83.6(11) 2_665 2_765
Ag5' Ag1 Ag3 Ag5' -107.6(8) 2_665 2_765
C9 Ag1 Ag3 Ag2 62.6(4) . 2_765
C1 Ag1 Ag3 Ag2 -126.0(4) 2_665 2_765
Ag4 Ag1 Ag3 Ag2 60.29(4) . 2_765
Ag4 Ag1 Ag3 Ag2 -65.18(5) 2_665 2_765
Ag5 Ag1 Ag3 Ag2 5.2(2) . 2_765
Ag2 Ag1 Ag3 Ag2 -57.35(4) . 2_765
Ag5 Ag1 Ag3 Ag2 -148.6(12) 2_665 2_765
Ag5' Ag1 Ag3 Ag2 -172.6(10) 2_665 2_765
C9 Ag1 Ag3 Ag2 119.9(4) . .
C1 Ag1 Ag3 Ag2 -68.6(4) 2_665 .
Ag4 Ag1 Ag3 Ag2 117.64(4) . .
Ag4 Ag1 Ag3 Ag2 -7.83(4) 2_665 .
Ag5 Ag1 Ag3 Ag2 62.6(2) . .
Ag5 Ag1 Ag3 Ag2 -91.2(12) 2_665 .
Ag5' Ag1 Ag3 Ag2 -115.3(10) 2_665 .
C9 Ag1 Ag3 Ag5 123.3(4) . 2_765
C1 Ag1 Ag3 Ag5 -65.2(4) 2_665 2_765
Ag4 Ag1 Ag3 Ag5 121.06(17) . 2_765
Ag4 Ag1 Ag3 Ag5 -4.40(17) 2_665 2_765
Ag5 Ag1 Ag3 Ag5 66.0(4) . 2_765
Ag2 Ag1 Ag3 Ag5 3.42(16) . 2_765
Ag5 Ag1 Ag3 Ag5 -87.8(12) 2_665 2_765
Ag5' Ag1 Ag3 Ag5 -111.9(10) 2_665 2_765
C9 Ag1 Ag4 O1 44.4(7) . .
C1 Ag1 Ag4 O1 -127.6(7) 2_665 .
Ag4 Ag1 Ag4 O1 177.6(6) 2_665 .
Ag3 Ag1 Ag4 O1 46.5(6) . .
Ag5 Ag1 Ag4 O1 107.3(7) . .
Ag2 Ag1 Ag4 O1 112.2(6) . .
Ag5 Ag1 Ag4 O1 -129.1(6) 2_665 .
Ag5' Ag1 Ag4 O1 -122.7(7) 2_665 .
C9 Ag1 Ag4 C1 -95.2(4) . .
C1 Ag1 Ag4 C1 92.9(4) 2_665 .
Ag4 Ag1 Ag4 C1 38.0(3) 2_665 .
Ag3 Ag1 Ag4 C1 -93.1(3) . .
Ag5 Ag1 Ag4 C1 -32.2(3) . .
Ag2 Ag1 Ag4 C1 -27.4(3) . .
Ag5 Ag1 Ag4 C1 91.3(3) 2_665 .
Ag5' Ag1 Ag4 C1 97.7(5) 2_665 .
C9 Ag1 Ag4 C17 138.1(4) . 2_665
C1 Ag1 Ag4 C17 -33.9(4) 2_665 2_665
Ag4 Ag1 Ag4 C17 -88.8(2) 2_665 2_665
Ag3 Ag1 Ag4 C17 140.1(2) . 2_665
Ag5 Ag1 Ag4 C17 -159.0(3) . 2_665
Ag2 Ag1 Ag4 C17 -154.2(2) . 2_665
Ag5 Ag1 Ag4 C17 -35.4(3) 2_665 2_665
Ag5' Ag1 Ag4 C17 -29.0(5) 2_665 2_665
C9 Ag1 Ag4 C18 111.5(5) . 2_665
C1 Ag1 Ag4 C18 -60.5(4) 2_665 2_665
Ag4 Ag1 Ag4 C18 -115.3(3) 2_665 2_665
Ag3 Ag1 Ag4 C18 113.6(3) . 2_665
Ag5 Ag1 Ag4 C18 174.5(4) . 2_665
Ag2 Ag1 Ag4 C18 179.3(3) . 2_665
Ag5 Ag1 Ag4 C18 -62.0(3) 2_665 2_665
Ag5' Ag1 Ag4 C18 -55.6(5) 2_665 2_665
C1 Ag1 Ag4 C9 -172.0(5) 2_665 .
Ag4 Ag1 Ag4 C9 133.2(4) 2_665 .
Ag3 Ag1 Ag4 C9 2.1(4) . .
Ag5 Ag1 Ag4 C9 62.9(4) . .
Ag2 Ag1 Ag4 C9 67.8(4) . .
Ag5 Ag1 Ag4 C9 -173.5(4) 2_665 .
Ag5' Ag1 Ag4 C9 -167.1(5) 2_665 .
C9 Ag1 Ag4 Ag1 -133.2(4) . 2_665
C1 Ag1 Ag4 Ag1 54.8(3) 2_665 2_665
Ag4 Ag1 Ag4 Ag1 0.0 2_665 2_665
Ag3 Ag1 Ag4 Ag1 -131.11(5) . 2_665
Ag5 Ag1 Ag4 Ag1 -70.2(2) . 2_665
Ag2 Ag1 Ag4 Ag1 -65.41(4) . 2_665
Ag5 Ag1 Ag4 Ag1 53.32(14) 2_665 2_665
Ag5' Ag1 Ag4 Ag1 59.7(4) 2_665 2_665
C9 Ag1 Ag4 Ag2 173.5(4) . 2_665
C1 Ag1 Ag4 Ag2 1.5(3) 2_665 2_665
Ag4 Ag1 Ag4 Ag2 -53.36(3) 2_665 2_665
Ag3 Ag1 Ag4 Ag2 175.54(4) . 2_665
Ag5 Ag1 Ag4 Ag2 -123.6(2) . 2_665
Ag2 Ag1 Ag4 Ag2 -118.77(4) . 2_665
Ag5 Ag1 Ag4 Ag2 -0.04(14) 2_665 2_665
Ag5' Ag1 Ag4 Ag2 6.4(4) 2_665 2_665
C9 Ag1 Ag4 Ag5 -62.9(4) . .
C1 Ag1 Ag4 Ag5 125.1(4) 2_665 .
Ag4 Ag1 Ag4 Ag5 70.2(2) 2_665 .
Ag3 Ag1 Ag4 Ag5 -60.9(2) . .
Ag2 Ag1 Ag4 Ag5 4.8(2) . .
Ag5 Ag1 Ag4 Ag5 123.56(19) 2_665 .
Ag5' Ag1 Ag4 Ag5 130.0(5) 2_665 .
C17 Ag2 Ag5 Ag5' 36(3) . .
C25 Ag2 Ag5 Ag5' -151(3) . .
Ag3 Ag2 Ag5 Ag5' -29(3) 2_765 .
Ag5 Ag2 Ag5 Ag5' -93(3) 2_765 .
Ag3 Ag2 Ag5 Ag5' -150(3) . .
Ag4 Ag2 Ag5 Ag5' 89(3) 2_665 .
Ag5' Ag2 Ag5 Ag5' -100(3) 2_765 .
Ag1 Ag2 Ag5 Ag5' 148(3) . .
C17 Ag2 Ag5 C1 -51.8(6) . .
C25 Ag2 Ag5 C1 121.2(7) . .
Ag3 Ag2 Ag5 C1 -116.0(6) 2_765 .
Ag5 Ag2 Ag5 C1 179.5(6) 2_765 .
Ag3 Ag2 Ag5 C1 123.1(6) . .
Ag4 Ag2 Ag5 C1 1.7(5) 2_665 .
Ag5' Ag2 Ag5 C1 172.2(8) 2_765 .
Ag1 Ag2 Ag5 C1 60.2(5) . .
Ag5' Ag2 Ag5 C1 -87(3) . .
C17 Ag2 Ag5 C25 92.1(5) . 2_765
C25 Ag2 Ag5 C25 -94.9(5) . 2_765
Ag3 Ag2 Ag5 C25 27.9(3) 2_765 2_765
Ag5 Ag2 Ag5 C25 -36.6(3) 2_765 2_765
Ag3 Ag2 Ag5 C25 -93.0(4) . 2_765
Ag4 Ag2 Ag5 C25 145.6(4) 2_665 2_765
Ag5' Ag2 Ag5 C25 -43.9(6) 2_765 2_765
Ag1 Ag2 Ag5 C25 -155.9(5) . 2_765
Ag5' Ag2 Ag5 C25 57(2) . 2_765
C17 Ag2 Ag5 C9 -149.4(5) . .
C25 Ag2 Ag5 C9 23.6(6) . .
Ag3 Ag2 Ag5 C9 146.4(4) 2_765 .
Ag5 Ag2 Ag5 C9 81.8(3) 2_765 .
Ag3 Ag2 Ag5 C9 25.4(3) . .
Ag4 Ag2 Ag5 C9 -96.0(3) 2_665 .
Ag5' Ag2 Ag5 C9 74.6(5) 2_765 .
Ag1 Ag2 Ag5 C9 -37.4(3) . .
Ag5' Ag2 Ag5 C9 175(3) . .
C25 Ag2 Ag5 C17 173.0(5) . .
Ag3 Ag2 Ag5 C17 -64.2(3) 2_765 .
Ag5 Ag2 Ag5 C17 -128.7(4) 2_765 .
Ag3 Ag2 Ag5 C17 174.9(4) . .
Ag4 Ag2 Ag5 C17 53.5(3) 2_665 .
Ag5' Ag2 Ag5 C17 -136.0(6) 2_765 .
Ag1 Ag2 Ag5 C17 112.0(4) . .
Ag5' Ag2 Ag5 C17 -36(3) . .
C17 Ag2 Ag5 Ag2 128.7(4) . 2_765
C25 Ag2 Ag5 Ag2 -58.3(4) . 2_765
Ag3 Ag2 Ag5 Ag2 64.53(10) 2_765 2_765
Ag5 Ag2 Ag5 Ag2 0.0 2_765 2_765
Ag3 Ag2 Ag5 Ag2 -56.41(11) . 2_765
Ag4 Ag2 Ag5 Ag2 -177.80(14) 2_665 2_765
Ag5' Ag2 Ag5 Ag2 -7.3(4) 2_765 2_765
Ag1 Ag2 Ag5 Ag2 -119.3(2) . 2_765
Ag5' Ag2 Ag5 Ag2 93(3) . 2_765
C17 Ag2 Ag5 Ag1 -112.0(4) . .
C25 Ag2 Ag5 Ag1 61.0(5) . .
Ag3 Ag2 Ag5 Ag1 -176.2(2) 2_765 .
Ag5 Ag2 Ag5 Ag1 119.3(2) 2_765 .
Ag3 Ag2 Ag5 Ag1 62.88(11) . .
Ag4 Ag2 Ag5 Ag1 -58.51(12) 2_665 .
Ag5' Ag2 Ag5 Ag1 112.0(5) 2_765 .
Ag5' Ag2 Ag5 Ag1 -148(3) . .
C17 Ag2 Ag5 Ag3 64.2(3) . 2_765
C25 Ag2 Ag5 Ag3 -122.8(4) . 2_765
Ag5 Ag2 Ag5 Ag3 -64.53(10) 2_765 2_765
Ag3 Ag2 Ag5 Ag3 -120.94(14) . 2_765
Ag4 Ag2 Ag5 Ag3 117.67(12) 2_665 2_765
Ag5' Ag2 Ag5 Ag3 -71.8(4) 2_765 2_765
Ag1 Ag2 Ag5 Ag3 176.2(2) . 2_765
Ag5' Ag2 Ag5 Ag3 29(3) . 2_765
C17 Ag2 Ag5 Ag4 -107.6(5) . .
C25 Ag2 Ag5 Ag4 65.4(6) . .
Ag3 Ag2 Ag5 Ag4 -171.8(4) 2_765 .
Ag5 Ag2 Ag5 Ag4 123.7(4) 2_765 .
Ag3 Ag2 Ag5 Ag4 67.3(3) . .
Ag4 Ag2 Ag5 Ag4 -54.1(3) 2_665 .
Ag5' Ag2 Ag5 Ag4 116.4(6) 2_765 .
Ag1 Ag2 Ag5 Ag4 4.4(2) . .
Ag5' Ag2 Ag5 Ag4 -143(3) . .
C17 Ag2 Ag5 Ag1 -53.4(4) . 2_665
C25 Ag2 Ag5 Ag1 119.5(4) . 2_665
Ag3 Ag2 Ag5 Ag1 -117.6(2) 2_765 2_665
Ag5 Ag2 Ag5 Ag1 177.8(3) 2_765 2_665
Ag3 Ag2 Ag5 Ag1 121.41(17) . 2_665
Ag4 Ag2 Ag5 Ag1 0.03(13) 2_665 2_665
Ag5' Ag2 Ag5 Ag1 170.5(5) 2_765 2_665
Ag1 Ag2 Ag5 Ag1 58.54(14) . 2_665
Ag5' Ag2 Ag5 Ag1 -89(3) . 2_665
C9 Ag1 Ag5 Ag5' -173(4) . .
C1 Ag1 Ag5 Ag5' 6(4) 2_665 .
Ag4 Ag1 Ag5 Ag5' 118(4) . .
Ag4 Ag1 Ag5 Ag5' 3(4) 2_665 .
Ag3 Ag1 Ag5 Ag5' -120(4) . .
Ag2 Ag1 Ag5 Ag5' -57(4) . .
Ag5 Ag1 Ag5 Ag5' 56(4) 2_665 .
Ag5' Ag1 Ag5 Ag5' 59(4) 2_665 .
C9 Ag1 Ag5 C1 100.6(6) . .
C1 Ag1 Ag5 C1 -79.9(6) 2_665 .
Ag4 Ag1 Ag5 C1 32.0(3) . .
Ag4 Ag1 Ag5 C1 -83.0(4) 2_665 .
Ag3 Ag1 Ag5 C1 154.1(4) . .
Ag2 Ag1 Ag5 C1 -143.3(5) . .
Ag5 Ag1 Ag5 C1 -30.2(3) 2_665 .
Ag5' Ag1 Ag5 C1 -26.5(6) 2_665 .
C9 Ag1 Ag5 C25 -66.7(10) . 2_765
C1 Ag1 Ag5 C25 112.8(10) 2_665 2_765
Ag4 Ag1 Ag5 C25 -135.4(11) . 2_765
Ag4 Ag1 Ag5 C25 109.6(10) 2_665 2_765
Ag3 Ag1 Ag5 C25 -13.3(10) . 2_765
Ag2 Ag1 Ag5 C25 49.3(9) . 2_765
Ag5 Ag1 Ag5 C25 162.4(11) 2_665 2_765
Ag5' Ag1 Ag5 C25 166.2(9) 2_665 2_765
C1 Ag1 Ag5 C9 179.5(5) 2_665 .
Ag4 Ag1 Ag5 C9 -68.6(4) . .
Ag4 Ag1 Ag5 C9 176.4(4) 2_665 .
Ag3 Ag1 Ag5 C9 53.5(4) . .
Ag2 Ag1 Ag5 C9 116.0(4) . .
Ag5 Ag1 Ag5 C9 -130.8(4) 2_665 .
Ag5' Ag1 Ag5 C9 -127.1(4) 2_665 .
C9 Ag1 Ag5 C17 -154.5(5) . .
C1 Ag1 Ag5 C17 25.0(6) 2_665 .
Ag4 Ag1 Ag5 C17 136.9(4) . .
Ag4 Ag1 Ag5 C17 21.9(3) 2_665 .
Ag3 Ag1 Ag5 C17 -101.1(3) . .
Ag2 Ag1 Ag5 C17 -38.5(3) . .
Ag5 Ag1 Ag5 C17 74.7(3) 2_665 .
Ag5' Ag1 Ag5 C17 78.4(4) 2_665 .
C9 Ag1 Ag5 Ag2 -58.7(4) . 2_765
C1 Ag1 Ag5 Ag2 120.8(5) 2_665 2_765
Ag4 Ag1 Ag5 Ag2 -127.3(4) . 2_765
Ag4 Ag1 Ag5 Ag2 117.7(3) 2_665 2_765
Ag3 Ag1 Ag5 Ag2 -5.2(2) . 2_765
Ag2 Ag1 Ag5 Ag2 57.4(2) . 2_765
Ag5 Ag1 Ag5 Ag2 170.5(4) 2_665 2_765
Ag5' Ag1 Ag5 Ag2 174.2(3) 2_665 2_765
C9 Ag1 Ag5 Ag2 -116.0(4) . .
C1 Ag1 Ag5 Ag2 63.5(4) 2_665 .
Ag4 Ag1 Ag5 Ag2 175.3(2) . .
Ag4 Ag1 Ag5 Ag2 60.32(12) 2_665 .
Ag3 Ag1 Ag5 Ag2 -62.60(11) . .
Ag5 Ag1 Ag5 Ag2 113.1(2) 2_665 .
Ag5' Ag1 Ag5 Ag2 116.8(3) 2_665 .
C9 Ag1 Ag5 Ag3 -119.6(5) . 2_765
C1 Ag1 Ag5 Ag3 59.9(6) 2_665 2_765
Ag4 Ag1 Ag5 Ag3 171.7(4) . 2_765
Ag4 Ag1 Ag5 Ag3 56.7(3) 2_665 2_765
Ag3 Ag1 Ag5 Ag3 -66.2(3) . 2_765
Ag2 Ag1 Ag5 Ag3 -3.6(2) . 2_765
Ag5 Ag1 Ag5 Ag3 109.5(4) 2_665 2_765
Ag5' Ag1 Ag5 Ag3 113.3(4) 2_665 2_765
C9 Ag1 Ag5 Ag4 68.6(4) . .
C1 Ag1 Ag5 Ag4 -111.9(4) 2_665 .
Ag4 Ag1 Ag5 Ag4 -114.99(12) 2_665 .
Ag3 Ag1 Ag5 Ag4 122.09(15) . .
Ag2 Ag1 Ag5 Ag4 -175.3(2) . .
Ag5 Ag1 Ag5 Ag4 -62.20(11) 2_665 .
Ag5' Ag1 Ag5 Ag4 -58.5(3) 2_665 .
C9 Ag1 Ag5 Ag1 130.8(4) . 2_665
C1 Ag1 Ag5 Ag1 -49.7(5) 2_665 2_665
Ag4 Ag1 Ag5 Ag1 62.20(11) . 2_665
Ag4 Ag1 Ag5 Ag1 -52.79(11) 2_665 2_665
Ag3 Ag1 Ag5 Ag1 -175.70(19) . 2_665
Ag2 Ag1 Ag5 Ag1 -113.1(2) . 2_665
Ag5 Ag1 Ag5 Ag1 0.0 2_665 2_665
Ag5' Ag1 Ag5 Ag1 3.7(4) 2_665 2_665
O1 Ag4 Ag5 Ag5' 86(4) . .
C1 Ag4 Ag5 Ag5' 3(4) . .
C17 Ag4 Ag5 Ag5' -99(4) 2_665 .
C18 Ag4 Ag5 Ag5' -138(4) 2_665 .
C9 Ag4 Ag5 Ag5' 177(4) . .
Ag1 Ag4 Ag5 Ag5' -130(4) . .
Ag1 Ag4 Ag5 Ag5' -47(4) 2_665 .
Ag2 Ag4 Ag5 Ag5' -44(4) 2_665 .
O1 Ag4 Ag5 C1 83.1(5) . .
C17 Ag4 Ag5 C1 -102.4(5) 2_665 .
C18 Ag4 Ag5 C1 -141.0(5) 2_665 .
C9 Ag4 Ag5 C1 173.8(6) . .
Ag1 Ag4 Ag5 C1 -133.4(5) . .
Ag1 Ag4 Ag5 C1 -49.7(4) 2_665 .
Ag2 Ag4 Ag5 C1 -47.0(5) 2_665 .
O1 Ag4 Ag5 C25 -1.2(8) . 2_765
C1 Ag4 Ag5 C25 -84.2(7) . 2_765
C17 Ag4 Ag5 C25 173.4(7) 2_665 2_765
C18 Ag4 Ag5 C25 134.8(7) 2_665 2_765
C9 Ag4 Ag5 C25 89.6(8) . 2_765
Ag1 Ag4 Ag5 C25 142.4(8) . 2_765
Ag1 Ag4 Ag5 C25 -133.9(7) 2_665 2_765
Ag2 Ag4 Ag5 C25 -131.2(7) 2_665 2_765
O1 Ag4 Ag5 C9 -90.8(4) . .
C1 Ag4 Ag5 C9 -173.8(6) . .
C17 Ag4 Ag5 C9 83.7(5) 2_665 .
C18 Ag4 Ag5 C9 45.1(6) 2_665 .
Ag1 Ag4 Ag5 C9 52.8(3) . .
Ag1 Ag4 Ag5 C9 136.4(4) 2_665 .
Ag2 Ag4 Ag5 C9 139.2(3) 2_665 .
O1 Ag4 Ag5 C17 163.3(5) . .
C1 Ag4 Ag5 C17 80.2(6) . .
C17 Ag4 Ag5 C17 -22.2(8) 2_665 .
C18 Ag4 Ag5 C17 -60.8(7) 2_665 .
C9 Ag4 Ag5 C17 -105.9(5) . .
Ag1 Ag4 Ag5 C17 -53.2(4) . .
Ag1 Ag4 Ag5 C17 30.5(4) 2_665 .
Ag2 Ag4 Ag5 C17 33.2(5) 2_665 .
O1 Ag4 Ag5 Ag2 -62.8(5) . 2_765
C1 Ag4 Ag5 Ag2 -145.8(6) . 2_765
C17 Ag4 Ag5 Ag2 111.8(5) 2_665 2_765
C18 Ag4 Ag5 Ag2 73.2(7) 2_665 2_765
C9 Ag4 Ag5 Ag2 28.0(4) . 2_765
Ag1 Ag4 Ag5 Ag2 80.8(3) . 2_765
Ag1 Ag4 Ag5 Ag2 164.5(4) 2_665 2_765
Ag2 Ag4 Ag5 Ag2 167.2(3) 2_665 2_765
O1 Ag4 Ag5 Ag2 -148.3(4) . .
C1 Ag4 Ag5 Ag2 128.7(6) . .
C17 Ag4 Ag5 Ag2 26.2(6) 2_665 .
C18 Ag4 Ag5 Ag2 -12.4(7) 2_665 .
C9 Ag4 Ag5 Ag2 -57.5(4) . .
Ag1 Ag4 Ag5 Ag2 -4.7(2) . .
Ag1 Ag4 Ag5 Ag2 79.0(4) 2_665 .
Ag2 Ag4 Ag5 Ag2 81.7(4) 2_665 .
O1 Ag4 Ag5 Ag1 -143.6(3) . .
C1 Ag4 Ag5 Ag1 133.4(5) . .
C17 Ag4 Ag5 Ag1 31.0(5) 2_665 .
C18 Ag4 Ag5 Ag1 -7.6(5) 2_665 .
C9 Ag4 Ag5 Ag1 -52.8(3) . .
Ag1 Ag4 Ag5 Ag1 83.68(16) 2_665 .
Ag2 Ag4 Ag5 Ag1 86.39(15) 2_665 .
O1 Ag4 Ag5 Ag3 163.3(17) . 2_765
C1 Ag4 Ag5 Ag3 80.2(18) . 2_765
C17 Ag4 Ag5 Ag3 -22(2) 2_665 2_765
C18 Ag4 Ag5 Ag3 -60.8(19) 2_665 2_765
C9 Ag4 Ag5 Ag3 -106.0(18) . 2_765
Ag1 Ag4 Ag5 Ag3 -53.2(17) . 2_765
Ag1 Ag4 Ag5 Ag3 30.5(17) 2_665 2_765
Ag2 Ag4 Ag5 Ag3 33.2(18) 2_665 2_765
O1 Ag4 Ag5 Ag1 132.8(3) . 2_665
C1 Ag4 Ag5 Ag1 49.7(4) . 2_665
C17 Ag4 Ag5 Ag1 -52.7(4) 2_665 2_665
C18 Ag4 Ag5 Ag1 -91.3(5) 2_665 2_665
C9 Ag4 Ag5 Ag1 -136.4(4) . 2_665
Ag1 Ag4 Ag5 Ag1 -83.68(16) . 2_665
Ag2 Ag4 Ag5 Ag1 2.71(18) 2_665 2_665
C1 Ag5 Ag5' C25 -129.9(14) . 2_765
C9 Ag5 Ag5' C25 20(33) . 2_765
C17 Ag5 Ag5' C25 120(2) . 2_765
Ag2 Ag5 Ag5' C25 23.9(18) 2_765 2_765
Ag2 Ag5 Ag5' C25 93.6(15) . 2_765
Ag1 Ag5 Ag5' C25 142(2) . 2_765
Ag3 Ag5 Ag5' C25 60(2) 2_765 2_765
Ag4 Ag5 Ag5' C25 -132(2) . 2_765
Ag1 Ag5 Ag5' C25 -168.7(13) 2_665 2_765
C25 Ag5 Ag5' C1 129.9(14) 2_765 .
C9 Ag5 Ag5' C1 150(32) . .
C17 Ag5 Ag5' C1 -109.9(12) . .
Ag2 Ag5 Ag5' C1 153.9(5) 2_765 .
Ag2 Ag5 Ag5' C1 -136.4(5) . .
Ag1 Ag5 Ag5' C1 -88(3) . .
Ag3 Ag5 Ag5' C1 -170(2) 2_765 .
Ag4 Ag5 Ag5' C1 -2(3) . .
Ag1 Ag5 Ag5' C1 -38.7(3) 2_665 .
C1 Ag5 Ag5' C17 109.9(12) . .
C25 Ag5 Ag5' C17 -120(2) 2_765 .
C9 Ag5 Ag5' C17 -100(32) . .
Ag2 Ag5 Ag5' C17 -96.2(13) 2_765 .
Ag2 Ag5 Ag5' C17 -26.5(16) . .
Ag1 Ag5 Ag5' C17 22(5) . .
Ag3 Ag5 Ag5' C17 -60(2) 2_765 .
Ag4 Ag5 Ag5' C17 108(3) . .
Ag1 Ag5 Ag5' C17 71.2(13) 2_665 .
C1 Ag5 Ag5' C26 -105(2) . 2_765
C25 Ag5 Ag5' C26 25.1(14) 2_765 2_765
C9 Ag5 Ag5' C26 45(33) . 2_765
C17 Ag5 Ag5' C26 145(3) . 2_765
Ag2 Ag5 Ag5' C26 49(3) 2_765 2_765
Ag2 Ag5 Ag5' C26 119(2) . 2_765
Ag1 Ag5 Ag5' C26 167.0(14) . 2_765
Ag3 Ag5 Ag5' C26 85(3) 2_765 2_765
Ag4 Ag5 Ag5' C26 -107(3) . 2_765
Ag1 Ag5 Ag5' C26 -144(2) 2_665 2_765
C1 Ag5 Ag5' C2 -26.0(4) . .
C25 Ag5 Ag5' C2 104.0(15) 2_765 .
C9 Ag5 Ag5' C2 124(32) . .
C17 Ag5 Ag5' C2 -135.9(13) . .
Ag2 Ag5 Ag5' C2 127.9(4) 2_765 .
Ag2 Ag5 Ag5' C2 -162.4(4) . .
Ag1 Ag5 Ag5' C2 -114(3) . .
Ag3 Ag5 Ag5' C2 164(2) 2_765 .
Ag4 Ag5 Ag5' C2 -28(3) . .
Ag1 Ag5 Ag5' C2 -64.7(3) 2_665 .
C1 Ag5 Ag5' Ag3 170(2) . 2_765
C25 Ag5 Ag5' Ag3 -60(2) 2_765 2_765
C9 Ag5 Ag5' Ag3 -40(33) . 2_765
C17 Ag5 Ag5' Ag3 60(2) . 2_765
Ag2 Ag5 Ag5' Ag3 -36(3) 2_765 2_765
Ag2 Ag5 Ag5' Ag3 33(3) . 2_765
Ag1 Ag5 Ag5' Ag3 82(4) . 2_765
Ag4 Ag5 Ag5' Ag3 167.6(7) . 2_765
Ag1 Ag5 Ag5' Ag3 131(2) 2_665 2_765
C1 Ag5 Ag5' Ag2 -153.9(5) . 2_765
C25 Ag5 Ag5' Ag2 -23.9(18) 2_765 2_765
C9 Ag5 Ag5' Ag2 -4(31) . 2_765
C17 Ag5 Ag5' Ag2 96.2(13) . 2_765
Ag2 Ag5 Ag5' Ag2 69.7(4) . 2_765
Ag1 Ag5 Ag5' Ag2 118(4) . 2_765
Ag3 Ag5 Ag5' Ag2 36(3) 2_765 2_765
Ag4 Ag5 Ag5' Ag2 -156(3) . 2_765
Ag1 Ag5 Ag5' Ag2 167.4(5) 2_665 2_765
C1 Ag5 Ag5' Ag2 136.4(5) . .
C25 Ag5 Ag5' Ag2 -93.6(15) 2_765 .
C9 Ag5 Ag5' Ag2 -73(32) . .
C17 Ag5 Ag5' Ag2 26.5(16) . .
Ag2 Ag5 Ag5' Ag2 -69.7(4) 2_765 .
Ag1 Ag5 Ag5' Ag2 48(3) . .
Ag3 Ag5 Ag5' Ag2 -33(3) 2_765 .
Ag4 Ag5 Ag5' Ag2 134(3) . .
Ag1 Ag5 Ag5' Ag2 97.7(4) 2_665 .
C1 Ag5 Ag5' Ag1 38.7(3) . 2_665
C25 Ag5 Ag5' Ag1 168.7(13) 2_765 2_665
C9 Ag5 Ag5' Ag1 -171(32) . 2_665
C17 Ag5 Ag5' Ag1 -71.2(13) . 2_665
Ag2 Ag5 Ag5' Ag1 -167.4(5) 2_765 2_665
Ag2 Ag5 Ag5' Ag1 -97.7(4) . 2_665
Ag1 Ag5 Ag5' Ag1 -49(3) . 2_665
Ag3 Ag5 Ag5' Ag1 -131(2) 2_765 2_665
Ag4 Ag5 Ag5' Ag1 36(3) . 2_665
C17 Ag2 Ag5' Ag5 -142(3) . .
C25 Ag2 Ag5' Ag5 31(3) . .
Ag3 Ag2 Ag5' Ag5 150(3) 2_765 .
Ag5 Ag2 Ag5' Ag5 89(3) 2_765 .
Ag3 Ag2 Ag5' Ag5 30(3) . .
Ag4 Ag2 Ag5' Ag5 -90(3) 2_665 .
Ag5' Ag2 Ag5' Ag5 82(3) 2_765 .
Ag1 Ag2 Ag5' Ag5 -31(3) . .
C17 Ag2 Ag5' C25 103.3(9) . 2_765
C25 Ag2 Ag5' C25 -83.6(10) . 2_765
Ag3 Ag2 Ag5' C25 34.7(6) 2_765 2_765
Ag5 Ag2 Ag5' C25 -25.6(8) 2_765 2_765
Ag5 Ag2 Ag5' C25 -115(3) . 2_765
Ag3 Ag2 Ag5' C25 -85.3(6) . 2_765
Ag4 Ag2 Ag5' C25 155.3(7) 2_665 2_765
Ag5' Ag2 Ag5' C25 -32.9(4) 2_765 2_765
Ag1 Ag2 Ag5' C25 -145.5(8) . 2_765
C17 Ag2 Ag5' C1 -68.3(11) . .
C25 Ag2 Ag5' C1 104.8(11) . .
Ag3 Ag2 Ag5' C1 -136.9(13) 2_765 .
Ag5 Ag2 Ag5' C1 162.8(11) 2_765 .
Ag5 Ag2 Ag5' C1 73(3) . .
Ag3 Ag2 Ag5' C1 103.1(12) . .
Ag4 Ag2 Ag5' C1 -16.3(11) 2_665 .
Ag5' Ag2 Ag5' C1 155.5(15) 2_765 .
Ag1 Ag2 Ag5' C1 42.9(11) . .
C25 Ag2 Ag5' C17 173.1(5) . .
Ag3 Ag2 Ag5' C17 -68.5(5) 2_765 .
Ag5 Ag2 Ag5' C17 -128.9(4) 2_765 .
Ag5 Ag2 Ag5' C17 142(3) . .
Ag3 Ag2 Ag5' C17 171.5(4) . .
Ag4 Ag2 Ag5' C17 52.0(4) 2_665 .
Ag5' Ag2 Ag5' C17 -136.1(6) 2_765 .
Ag1 Ag2 Ag5' C17 111.2(4) . .
C17 Ag2 Ag5' C26 86.9(10) . 2_765
C25 Ag2 Ag5' C26 -100.0(10) . 2_765
Ag3 Ag2 Ag5' C26 18.4(7) 2_765 2_765
Ag5 Ag2 Ag5' C26 -42.0(9) 2_765 2_765
Ag5 Ag2 Ag5' C26 -131(3) . 2_765
Ag3 Ag2 Ag5' C26 -101.6(8) . 2_765
Ag4 Ag2 Ag5' C26 138.9(9) 2_665 2_765
Ag5' Ag2 Ag5' C26 -49.2(6) 2_765 2_765
Ag1 Ag2 Ag5' C26 -161.9(9) . 2_765
C17 Ag2 Ag5' C2 -82(2) . .
C25 Ag2 Ag5' C2 91(2) . .
Ag3 Ag2 Ag5' C2 -151(2) 2_765 .
Ag5 Ag2 Ag5' C2 149(2) 2_765 .
Ag5 Ag2 Ag5' C2 60(3) . .
Ag3 Ag2 Ag5' C2 89(2) . .
Ag4 Ag2 Ag5' C2 -30(2) 2_665 .
Ag5' Ag2 Ag5' C2 142(3) 2_765 .
Ag1 Ag2 Ag5' C2 29(2) . .
C17 Ag2 Ag5' Ag3 68.5(5) . 2_765
C25 Ag2 Ag5' Ag3 -118.4(5) . 2_765
Ag5 Ag2 Ag5' Ag3 -60.3(3) 2_765 2_765
Ag5 Ag2 Ag5' Ag3 -150(3) . 2_765
Ag3 Ag2 Ag5' Ag3 -120.01(11) . 2_765
Ag4 Ag2 Ag5' Ag3 120.6(2) 2_665 2_765
Ag5' Ag2 Ag5' Ag3 -67.59(18) 2_765 2_765
Ag1 Ag2 Ag5' Ag3 179.7(2) . 2_765
C17 Ag2 Ag5' Ag2 136.1(6) . 2_765
C25 Ag2 Ag5' Ag2 -50.8(6) . 2_765
Ag3 Ag2 Ag5' Ag2 67.59(18) 2_765 2_765
Ag5 Ag2 Ag5' Ag2 7.3(4) 2_765 2_765
Ag5 Ag2 Ag5' Ag2 -82(3) . 2_765
Ag3 Ag2 Ag5' Ag2 -52.4(3) . 2_765
Ag4 Ag2 Ag5' Ag2 -171.8(4) 2_665 2_765
Ag5' Ag2 Ag5' Ag2 0.0 2_765 2_765
Ag1 Ag2 Ag5' Ag2 -112.7(4) . 2_765
C17 Ag2 Ag5' Ag1 -57.9(4) . 2_665
C25 Ag2 Ag5' Ag1 115.2(5) . 2_665
Ag3 Ag2 Ag5' Ag1 -126.4(6) 2_765 2_665
Ag5 Ag2 Ag5' Ag1 173.2(4) 2_765 2_665
Ag5 Ag2 Ag5' Ag1 84(3) . 2_665
Ag3 Ag2 Ag5' Ag1 113.6(5) . 2_665
Ag4 Ag2 Ag5' Ag1 -5.9(4) 2_665 2_665
Ag5' Ag2 Ag5' Ag1 166.0(7) 2_765 2_665
Ag1 Ag2 Ag5' Ag1 53.3(3) . 2_665
O1 Ag4 C1 C2 -28.7(9) . .
C17 Ag4 C1 C2 -145.3(8) 2_665 .
C18 Ag4 C1 C2 -159.9(9) 2_665 .
C9 Ag4 C1 C2 87.6(8) . .
Ag1 Ag4 C1 C2 130.9(8) . .
Ag1 Ag4 C1 C2 -171.2(10) 2_665 .
Ag2 Ag4 C1 C2 -123.8(8) 2_665 .
Ag5 Ag4 C1 C2 92.3(9) . .
O1 Ag4 C1 Ag1 142.5(4) . 2_665
C17 Ag4 C1 Ag1 25.9(5) 2_665 2_665
C18 Ag4 C1 Ag1 11.3(9) 2_665 2_665
C9 Ag4 C1 Ag1 -101.3(3) . 2_665
Ag1 Ag4 C1 Ag1 -57.9(3) . 2_665
Ag2 Ag4 C1 Ag1 47.4(3) 2_665 2_665
Ag5 Ag4 C1 Ag1 -96.5(5) . 2_665
O1 Ag4 C1 Ag5' -121.3(4) . .
C17 Ag4 C1 Ag5' 122.0(4) 2_665 .
C18 Ag4 C1 Ag5' 107.4(8) 2_665 .
C9 Ag4 C1 Ag5' -5.1(4) . .
Ag1 Ag4 C1 Ag5' 38.3(3) . .
Ag1 Ag4 C1 Ag5' 96.2(4) 2_665 .
Ag2 Ag4 C1 Ag5' 143.6(3) 2_665 .
Ag5 Ag4 C1 Ag5' -0.4(4) . .
O1 Ag4 C1 Ag5 -121.0(5) . .
C17 Ag4 C1 Ag5 122.4(5) 2_665 .
C18 Ag4 C1 Ag5 107.8(8) 2_665 .
C9 Ag4 C1 Ag5 -4.7(5) . .
Ag1 Ag4 C1 Ag5 38.6(4) . .
Ag1 Ag4 C1 Ag5 96.5(5) 2_665 .
Ag2 Ag4 C1 Ag5 143.9(4) 2_665 .
Ag5 Ag5' C1 C2 -98(3) . .
C25 Ag5' C1 C2 21.4(15) 2_765 .
C17 Ag5' C1 C2 149.7(11) . .
C26 Ag5' C1 C2 33.3(11) 2_765 .
Ag3 Ag5' C1 C2 95.8(10) 2_765 .
Ag2 Ag5' C1 C2 -39(2) 2_765 .
Ag2 Ag5' C1 C2 -169.1(13) . .
Ag1 Ag5' C1 C2 174.2(10) 2_665 .
Ag5 Ag5' C1 Ag1 88(3) . 2_665
C25 Ag5' C1 Ag1 -152.7(11) 2_765 2_665
C17 Ag5' C1 Ag1 -24.4(9) . 2_665
C26 Ag5' C1 Ag1 -140.9(7) 2_765 2_665
C2 Ag5' C1 Ag1 -174.2(10) . 2_665
Ag3 Ag5' C1 Ag1 -78.4(8) 2_765 2_665
Ag2 Ag5' C1 Ag1 147.0(16) 2_765 2_665
Ag2 Ag5' C1 Ag1 16.8(13) . 2_665
Ag5 Ag5' C1 Ag4 2(3) . .
C25 Ag5' C1 Ag4 121.5(11) 2_765 .
C17 Ag5' C1 Ag4 -110.2(8) . .
C26 Ag5' C1 Ag4 133.4(7) 2_765 .
C2 Ag5' C1 Ag4 100.1(9) . .
Ag3 Ag5' C1 Ag4 -164.1(5) 2_765 .
Ag2 Ag5' C1 Ag4 61.3(17) 2_765 .
Ag2 Ag5' C1 Ag4 -69.0(12) . .
Ag1 Ag5' C1 Ag4 -85.7(4) 2_665 .
C25 Ag5' C1 Ag5 119(3) 2_765 .
C17 Ag5' C1 Ag5 -112(3) . .
C26 Ag5' C1 Ag5 131(3) 2_765 .
C2 Ag5' C1 Ag5 98(3) . .
Ag3 Ag5' C1 Ag5 -166(3) 2_765 .
Ag2 Ag5' C1 Ag5 59(3) 2_765 .
Ag2 Ag5' C1 Ag5 -71(3) . .
Ag1 Ag5' C1 Ag5 -88(3) 2_665 .
Ag5' Ag5 C1 C2 83(3) . .
C25 Ag5 C1 C2 35.3(11) 2_765 .
C9 Ag5 C1 C2 -94.8(9) . .
C17 Ag5 C1 C2 140.1(8) . .
Ag2 Ag5 C1 C2 -8.2(14) 2_765 .
Ag2 Ag5 C1 C2 172.8(8) . .
Ag1 Ag5 C1 C2 -136.9(8) . .
Ag3 Ag5 C1 C2 92.2(10) 2_765 .
Ag4 Ag5 C1 C2 -99.7(9) . .
Ag1 Ag5 C1 C2 175.5(10) 2_665 .
Ag5' Ag5 C1 Ag1 -93(3) . 2_665
C25 Ag5 C1 Ag1 -140.2(6) 2_765 2_665
C9 Ag5 C1 Ag1 89.7(5) . 2_665
C17 Ag5 C1 Ag1 -35.4(5) . 2_665
Ag2 Ag5 C1 Ag1 176.3(7) 2_765 2_665
Ag2 Ag5 C1 Ag1 -2.7(7) . 2_665
Ag1 Ag5 C1 Ag1 47.6(4) . 2_665
Ag3 Ag5 C1 Ag1 -83.3(6) 2_765 2_665
Ag4 Ag5 C1 Ag1 84.8(4) . 2_665
Ag5' Ag5 C1 Ag4 -178(3) . .
C25 Ag5 C1 Ag4 135.1(6) 2_765 .
C9 Ag5 C1 Ag4 4.9(5) . .
C17 Ag5 C1 Ag4 -120.2(4) . .
Ag2 Ag5 C1 Ag4 91.5(9) 2_765 .
Ag2 Ag5 C1 Ag4 -87.4(6) . .
Ag1 Ag5 C1 Ag4 -37.2(3) . .
Ag3 Ag5 C1 Ag4 -168.0(5) 2_765 .
Ag1 Ag5 C1 Ag4 -84.8(4) 2_665 .
C25 Ag5 C1 Ag5' -47(2) 2_765 .
C9 Ag5 C1 Ag5' -177(3) . .
C17 Ag5 C1 Ag5' 58(3) . .
Ag2 Ag5 C1 Ag5' -91(2) 2_765 .
Ag2 Ag5 C1 Ag5' 90(3) . .
Ag1 Ag5 C1 Ag5' 141(3) . .
Ag3 Ag5 C1 Ag5' 10(2) 2_765 .
Ag4 Ag5 C1 Ag5' 178(3) . .
Ag1 Ag5 C1 Ag5' 93(3) 2_665 .
Ag1 C1 C2 C3 -17(21) 2_665 .
Ag4 C1 C2 C3 102(16) . .
Ag5' C1 C2 C3 -162(16) . .
Ag5 C1 C2 C3 -171(16) . .
Ag1 C1 C2 Ag5' 145(6) 2_665 .
Ag4 C1 C2 Ag5' -95.4(7) . .
Ag5 C1 C2 Ag5' -8.7(5) . .
Ag5 Ag5' C2 C1 81(3) . .
C25 Ag5' C2 C1 -162.7(12) 2_765 .
C17 Ag5' C2 C1 -39.5(13) . .
C26 Ag5' C2 C1 -147.5(11) 2_765 .
Ag3 Ag5' C2 C1 -117.9(10) 2_765 .
Ag2 Ag5' C2 C1 156.7(14) 2_765 .
Ag2 Ag5' C2 C1 23(2) . .
Ag1 Ag5' C2 C1 -4.0(7) 2_665 .
Ag5 Ag5' C2 C3 -101(3) . .
C25 Ag5' C2 C3 15.6(14) 2_765 .
C1 Ag5' C2 C3 178.4(15) . .
C17 Ag5' C2 C3 138.9(11) . .
C26 Ag5' C2 C3 30.9(12) 2_765 .
Ag3 Ag5' C2 C3 60.4(13) 2_765 .
Ag2 Ag5' C2 C3 -24.9(16) 2_765 .
Ag2 Ag5' C2 C3 -159(2) . .
Ag1 Ag5' C2 C3 174.3(10) 2_665 .
C1 C2 C3 C4 22(16) . .
Ag5' C2 C3 C4 -138.9(9) . .
C1 C2 C3 C8 -153(16) . .
Ag5' C2 C3 C8 45.9(13) . .
C8 C3 C4 C5 0.0 . .
C2 C3 C4 C5 -175.3(9) . .
C3 C4 C5 C6 0.0 . .
C4 C5 C6 C7 0.0 . .
C5 C6 C7 C8 0.0 . .
C6 C7 C8 C3 0.0 . .
C4 C3 C8 C7 0.0 . .
C2 C3 C8 C7 175.2(9) . .
C1 Ag1 C9 C10 1(5) 2_665 .
Ag4 Ag1 C9 C10 -103(2) . .
Ag4 Ag1 C9 C10 172.9(19) 2_665 .
Ag3 Ag1 C9 C10 80(2) . .
Ag5 Ag1 C9 C10 178(2) . .
Ag2 Ag1 C9 C10 128(2) . .
Ag5 Ag1 C9 C10 -94(2) 2_665 .
Ag5' Ag1 C9 C10 -85(2) 2_665 .
C1 Ag1 C9 Ag3 -79(3) 2_665 .
Ag4 Ag1 C9 Ag3 177.5(4) . .
Ag4 Ag1 C9 Ag3 93.1(4) 2_665 .
Ag5 Ag1 C9 Ag3 98.3(4) . .
Ag2 Ag1 C9 Ag3 47.9(2) . .
Ag5 Ag1 C9 Ag3 -173.3(2) 2_665 .
Ag5' Ag1 C9 Ag3 -164.5(6) 2_665 .
C1 Ag1 C9 Ag5 -177(3) 2_665 .
Ag4 Ag1 C9 Ag5 79.2(3) . .
Ag4 Ag1 C9 Ag5 -5.2(5) 2_665 .
Ag3 Ag1 C9 Ag5 -98.3(4) . .
Ag2 Ag1 C9 Ag5 -50.3(3) . .
Ag5 Ag1 C9 Ag5 88.4(5) 2_665 .
Ag5' Ag1 C9 Ag5 97.2(7) 2_665 .
C1 Ag1 C9 Ag4 104(3) 2_665 .
Ag4 Ag1 C9 Ag4 -84.4(4) 2_665 .
Ag3 Ag1 C9 Ag4 -177.5(4) . .
Ag5 Ag1 C9 Ag4 -79.2(3) . .
Ag2 Ag1 C9 Ag4 -129.57(18) . .
Ag5 Ag1 C9 Ag4 9.1(5) 2_665 .
Ag5' Ag1 C9 Ag4 18.0(7) 2_665 .
O2 Ag3 C9 C10 -56.3(8) . .
C25 Ag3 C9 C10 177.5(7) . .
C17 Ag3 C9 C10 55.8(8) 2_765 .
Ag5' Ag3 C9 C10 117.5(7) 2_765 .
Ag2 Ag3 C9 C10 84.6(7) 2_765 .
Ag2 Ag3 C9 C10 154.4(7) . .
Ag1 Ag3 C9 C10 -155.7(9) . .
Ag5 Ag3 C9 C10 117.7(7) 2_765 .
O2 Ag3 C9 Ag1 99.4(5) . .
C25 Ag3 C9 Ag1 -26.8(6) . .
C17 Ag3 C9 Ag1 -148.5(3) 2_765 .
C10 Ag3 C9 Ag1 155.7(9) . .
Ag5' Ag3 C9 Ag1 -86.8(4) 2_765 .
Ag2 Ag3 C9 Ag1 -119.7(3) 2_765 .
Ag2 Ag3 C9 Ag1 -49.9(3) . .
Ag5 Ag3 C9 Ag1 -86.6(5) 2_765 .
O2 Ag3 C9 Ag5 -178.8(5) . .
C25 Ag3 C9 Ag5 55.0(6) . .
C17 Ag3 C9 Ag5 -66.6(5) 2_765 .
C10 Ag3 C9 Ag5 -122.5(9) . .
Ag5' Ag3 C9 Ag5 -5.0(5) 2_765 .
Ag2 Ag3 C9 Ag5 -37.9(3) 2_765 .
Ag2 Ag3 C9 Ag5 31.9(4) . .
Ag1 Ag3 C9 Ag5 81.8(4) . .
Ag5 Ag3 C9 Ag5 -4.8(7) 2_765 .
O2 Ag3 C9 Ag4 108.0(18) . .
C25 Ag3 C9 Ag4 -18(2) . .
C17 Ag3 C9 Ag4 -139.8(17) 2_765 .
C10 Ag3 C9 Ag4 164(2) . .
Ag5' Ag3 C9 Ag4 -78.2(18) 2_765 .
Ag2 Ag3 C9 Ag4 -111.1(18) 2_765 .
Ag2 Ag3 C9 Ag4 -41.3(17) . .
Ag1 Ag3 C9 Ag4 8.6(15) . .
Ag5 Ag3 C9 Ag4 -78.0(18) 2_765 .
Ag5' Ag5 C9 C10 -52(32) . .
C1 Ag5 C9 C10 97.5(10) . .
C25 Ag5 C9 C10 -33.2(12) 2_765 .
C17 Ag5 C9 C10 -149.3(10) . .
Ag2 Ag5 C9 C10 -56.1(10) 2_765 .
Ag2 Ag5 C9 C10 -126.1(10) . .
Ag1 Ag5 C9 C10 -179.0(12) . .
Ag3 Ag5 C9 C10 -89.4(11) 2_765 .
Ag4 Ag5 C9 C10 102.0(10) . .
Ag1 Ag5 C9 C10 136.6(9) 2_665 .
Ag5' Ag5 C9 Ag1 127(32) . .
C1 Ag5 C9 Ag1 -83.5(5) . .
C25 Ag5 C9 Ag1 145.8(6) 2_765 .
C17 Ag5 C9 Ag1 29.7(6) . .
Ag2 Ag5 C9 Ag1 122.9(3) 2_765 .
Ag2 Ag5 C9 Ag1 52.9(3) . .
Ag3 Ag5 C9 Ag1 89.6(6) 2_765 .
Ag4 Ag5 C9 Ag1 -79.0(3) . .
Ag1 Ag5 C9 Ag1 -44.4(3) 2_665 .
Ag5' Ag5 C9 Ag3 42(32) . .
C1 Ag5 C9 Ag3 -168.5(4) . .
C25 Ag5 C9 Ag3 60.8(6) 2_765 .
C17 Ag5 C9 Ag3 -55.2(6) . .
Ag2 Ag5 C9 Ag3 37.9(3) 2_765 .
Ag2 Ag5 C9 Ag3 -32.1(3) . .
Ag1 Ag5 C9 Ag3 -85.0(4) . .
Ag3 Ag5 C9 Ag3 4.6(7) 2_765 .
Ag4 Ag5 C9 Ag3 -163.9(4) . .
Ag1 Ag5 C9 Ag3 -129.4(3) 2_665 .
Ag5' Ag5 C9 Ag4 -154(32) . .
C1 Ag5 C9 Ag4 -4.5(4) . .
C25 Ag5 C9 Ag4 -135.2(6) 2_765 .
C17 Ag5 C9 Ag4 108.7(5) . .
Ag2 Ag5 C9 Ag4 -158.1(3) 2_765 .
Ag2 Ag5 C9 Ag4 131.9(3) . .
Ag1 Ag5 C9 Ag4 79.0(3) . .
Ag3 Ag5 C9 Ag4 168.5(5) 2_765 .
Ag1 Ag5 C9 Ag4 34.6(3) 2_665 .
O1 Ag4 C9 C10 -2.5(9) . .
C1 Ag4 C9 C10 -115.9(8) . .
C17 Ag4 C9 C10 108.3(8) 2_665 .
C18 Ag4 C9 C10 89.8(8) 2_665 .
Ag1 Ag4 C9 C10 154.8(10) . .
Ag1 Ag4 C9 C10 -159.9(8) 2_665 .
Ag2 Ag4 C9 C10 142.9(6) 2_665 .
Ag5 Ag4 C9 C10 -120.4(9) . .
O1 Ag4 C9 Ag1 -157.4(4) . .
C1 Ag4 C9 Ag1 89.3(4) . .
C17 Ag4 C9 Ag1 -46.5(4) 2_665 .
C18 Ag4 C9 Ag1 -65.1(4) 2_665 .
Ag1 Ag4 C9 Ag1 45.3(3) 2_665 .
Ag2 Ag4 C9 Ag1 -12.0(6) 2_665 .
Ag5 Ag4 C9 Ag1 84.8(4) . .
O1 Ag4 C9 Ag3 -166.2(17) . .
C1 Ag4 C9 Ag3 80.5(18) . .
C17 Ag4 C9 Ag3 -55.3(18) 2_665 .
C18 Ag4 C9 Ag3 -73.9(18) 2_665 .
Ag1 Ag4 C9 Ag3 -8.8(15) . .
Ag1 Ag4 C9 Ag3 36.5(18) 2_665 .
Ag2 Ag4 C9 Ag3 -21(2) 2_665 .
Ag5 Ag4 C9 Ag3 76.0(17) . .
O1 Ag4 C9 Ag5 117.9(4) . .
C1 Ag4 C9 Ag5 4.5(4) . .
C17 Ag4 C9 Ag5 -131.3(4) 2_665 .
C18 Ag4 C9 Ag5 -149.8(4) 2_665 .
Ag1 Ag4 C9 Ag5 -84.8(4) . .
Ag1 Ag4 C9 Ag5 -39.5(3) 2_665 .
Ag2 Ag4 C9 Ag5 -96.7(5) 2_665 .
Ag1 C9 C10 C11 125(10) . .
Ag3 C9 C10 C11 -156(11) . .
Ag5 C9 C10 C11 -57(11) . .
Ag4 C9 C10 C11 29(11) . .
Ag1 C9 C10 Ag3 -79(2) . .
Ag5 C9 C10 Ag3 98.6(8) . .
Ag4 C9 C10 Ag3 -175.4(7) . .
O2 Ag3 C10 C9 128.9(8) . .
C25 Ag3 C10 C9 -4.3(12) . .
C17 Ag3 C10 C9 -131.0(7) 2_765 .
Ag5' Ag3 C10 C9 -95.2(9) 2_765 .
Ag2 Ag3 C10 C9 -91.6(7) 2_765 .
Ag2 Ag3 C10 C9 -27.6(8) . .
Ag1 Ag3 C10 C9 17.4(7) . .
Ag5 Ag3 C10 C9 -90.0(8) 2_765 .
O2 Ag3 C10 C11 -54.0(8) . .
C9 Ag3 C10 C11 177.1(13) . .
C25 Ag3 C10 C11 172.8(8) . .
C17 Ag3 C10 C11 46.1(8) 2_765 .
Ag5' Ag3 C10 C11 81.9(10) 2_765 .
Ag2 Ag3 C10 C11 85.5(8) 2_765 .
Ag2 Ag3 C10 C11 149.5(7) . .
Ag1 Ag3 C10 C11 -165.5(8) . .
Ag5 Ag3 C10 C11 87.1(9) 2_765 .
C9 C10 C11 C12 -18(11) . .
Ag3 C10 C11 C12 -172.6(5) . .
C9 C10 C11 C16 165(10) . .
Ag3 C10 C11 C16 10.7(10) . .
C16 C11 C12 C13 0.0 . .
C10 C11 C12 C13 -176.6(9) . .
C11 C12 C13 C14 0.0 . .
C12 C13 C14 C15 0.0 . .
C13 C14 C15 C16 0.0 . .
C14 C15 C16 C11 0.0 . .
C12 C11 C16 C15 0.0 . .
C10 C11 C16 C15 176.7(9) . .
C25 Ag2 C17 C18 16(5) . .
Ag3 Ag2 C17 C18 -127(3) 2_765 .
Ag5 Ag2 C17 C18 -117(3) 2_765 .
Ag5 Ag2 C17 C18 153(3) . .
Ag3 Ag2 C17 C18 146(2) . .
Ag4 Ag2 C17 C18 53(3) 2_665 .
Ag5' Ag2 C17 C18 -120(3) 2_765 .
Ag1 Ag2 C17 C18 101(3) . .
Ag5' Ag2 C17 C18 158(3) . .
C25 Ag2 C17 Ag5' -142(3) . .
Ag3 Ag2 C17 Ag5' 75.2(4) 2_765 .
Ag5 Ag2 C17 Ag5' 85.3(6) 2_765 .
Ag5 Ag2 C17 Ag5' -4.8(4) . .
Ag3 Ag2 C17 Ag5' -11.7(6) . .
Ag4 Ag2 C17 Ag5' -105.2(5) 2_665 .
Ag5' Ag2 C17 Ag5' 81.5(7) 2_765 .
Ag1 Ag2 C17 Ag5' -57.4(4) . .
C25 Ag2 C17 Ag4 -37(3) . 2_665
Ag3 Ag2 C17 Ag4 -179.5(4) 2_765 2_665
Ag5 Ag2 C17 Ag4 -169.5(3) 2_765 2_665
Ag5 Ag2 C17 Ag4 100.4(4) . 2_665
Ag3 Ag2 C17 Ag4 93.5(3) . 2_665
Ag5' Ag2 C17 Ag4 -173.3(3) 2_765 2_665
Ag1 Ag2 C17 Ag4 47.9(2) . 2_665
Ag5' Ag2 C17 Ag4 105.2(5) . 2_665
C25 Ag2 C17 Ag3 142(3) . 2_765
Ag5 Ag2 C17 Ag3 10.1(6) 2_765 2_765
Ag5 Ag2 C17 Ag3 -80.1(3) . 2_765
Ag3 Ag2 C17 Ag3 -87.0(3) . 2_765
Ag4 Ag2 C17 Ag3 179.5(4) 2_665 2_765
Ag5' Ag2 C17 Ag3 6.2(6) 2_765 2_765
Ag1 Ag2 C17 Ag3 -132.6(2) . 2_765
Ag5' Ag2 C17 Ag3 -75.2(4) . 2_765
C25 Ag2 C17 Ag5 -138(3) . .
Ag3 Ag2 C17 Ag5 80.1(3) 2_765 .
Ag5 Ag2 C17 Ag5 90.2(5) 2_765 .
Ag3 Ag2 C17 Ag5 -6.9(5) . .
Ag4 Ag2 C17 Ag5 -100.4(4) 2_665 .
Ag5' Ag2 C17 Ag5 86.3(6) 2_765 .
Ag1 Ag2 C17 Ag5 -52.5(3) . .
Ag5' Ag2 C17 Ag5 4.8(4) . .
Ag5 Ag5' C17 C18 -129(3) . .
C25 Ag5' C17 C18 104.2(11) 2_765 .
C1 Ag5' C17 C18 -35.9(14) . .
C26 Ag5' C17 C18 77.7(11) 2_765 .
C2 Ag5' C17 C18 -18.5(17) . .
Ag3 Ag5' C17 C18 108.0(10) 2_765 .
Ag2 Ag5' C17 C18 148.5(10) 2_765 .
Ag2 Ag5' C17 C18 -170.7(12) . .
Ag1 Ag5' C17 C18 -51.4(10) 2_665 .
Ag5 Ag5' C17 Ag2 41(3) . .
C25 Ag5' C17 Ag2 -85.1(7) 2_765 .
C1 Ag5' C17 Ag2 134.8(9) . .
C26 Ag5' C17 Ag2 -111.6(7) 2_765 .
C2 Ag5' C17 Ag2 152.2(11) . .
Ag3 Ag5' C17 Ag2 -81.3(3) 2_765 .
Ag2 Ag5' C17 Ag2 -40.8(6) 2_765 .
Ag1 Ag5' C17 Ag2 119.3(4) 2_665 .
Ag5 Ag5' C17 Ag4 -42(3) . 2_665
C25 Ag5' C17 Ag4 -168.0(6) 2_765 2_665
C1 Ag5' C17 Ag4 51.9(10) . 2_665
C26 Ag5' C17 Ag4 165.5(6) 2_765 2_665
C2 Ag5' C17 Ag4 69.3(12) . 2_665
Ag3 Ag5' C17 Ag4 -164.2(5) 2_765 2_665
Ag2 Ag5' C17 Ag4 -123.8(5) 2_765 2_665
Ag2 Ag5' C17 Ag4 -82.9(4) . 2_665
Ag1 Ag5' C17 Ag4 36.4(4) 2_665 2_665
Ag5 Ag5' C17 Ag3 123(3) . 2_765
C25 Ag5' C17 Ag3 -3.8(6) 2_765 2_765
C1 Ag5' C17 Ag3 -143.9(9) . 2_765
C26 Ag5' C17 Ag3 -30.3(6) 2_765 2_765
C2 Ag5' C17 Ag3 -126.5(12) . 2_765
Ag2 Ag5' C17 Ag3 40.5(4) 2_765 2_765
Ag2 Ag5' C17 Ag3 81.3(3) . 2_765
Ag1 Ag5' C17 Ag3 -159.4(4) 2_665 2_765
C25 Ag5' C17 Ag5 -126(3) 2_765 .
C1 Ag5' C17 Ag5 93(3) . .
C26 Ag5' C17 Ag5 -153(3) 2_765 .
C2 Ag5' C17 Ag5 111(3) . .
Ag3 Ag5' C17 Ag5 -123(3) 2_765 .
Ag2 Ag5' C17 Ag5 -82(3) 2_765 .
Ag2 Ag5' C17 Ag5 -41(3) . .
Ag1 Ag5' C17 Ag5 78(3) 2_665 .
Ag5' Ag5 C17 C18 54(3) . .
C1 Ag5 C17 C18 -22.3(11) . .
C25 Ag5 C17 C18 100.1(11) 2_765 .
C9 Ag5 C17 C18 -132.2(10) . .
Ag2 Ag5 C17 C18 144.3(10) 2_765 .
Ag2 Ag5 C17 C18 -168.3(12) . .
Ag1 Ag5 C17 C18 -112.4(10) . .
Ag3 Ag5 C17 C18 109.7(11) 2_765 .
Ag4 Ag5 C17 C18 -70.3(11) . .
Ag1 Ag5 C17 C18 -44.6(10) 2_665 .
Ag5' Ag5 C17 Ag2 -138(3) . .
C1 Ag5 C17 Ag2 146.0(4) . .
C25 Ag5 C17 Ag2 -91.6(4) 2_765 .
C9 Ag5 C17 Ag2 36.1(6) . .
Ag2 Ag5 C17 Ag2 -47.5(3) 2_765 .
Ag1 Ag5 C17 Ag2 55.8(3) . .
Ag3 Ag5 C17 Ag2 -82.1(3) 2_765 .
Ag4 Ag5 C17 Ag2 98.0(4) . .
Ag1 Ag5 C17 Ag2 123.7(3) 2_665 .
C1 Ag5 C17 Ag5' -76(3) . .
C25 Ag5 C17 Ag5' 46(3) 2_765 .
C9 Ag5 C17 Ag5' 174(3) . .
Ag2 Ag5 C17 Ag5' 90(3) 2_765 .
Ag2 Ag5 C17 Ag5' 138(3) . .
Ag1 Ag5 C17 Ag5' -166(3) . .
Ag3 Ag5 C17 Ag5' 56(3) 2_765 .
Ag4 Ag5 C17 Ag5' -124(3) . .
Ag1 Ag5 C17 Ag5' -98(3) 2_665 .
Ag5' Ag5 C17 Ag4 139(3) . 2_665
C1 Ag5 C17 Ag4 63.4(5) . 2_665
C25 Ag5 C17 Ag4 -174.2(4) 2_765 2_665
C9 Ag5 C17 Ag4 -46.5(6) . 2_665
Ag2 Ag5 C17 Ag4 -130.1(3) 2_765 2_665
Ag2 Ag5 C17 Ag4 -82.6(4) . 2_665
Ag1 Ag5 C17 Ag4 -26.8(3) . 2_665
Ag3 Ag5 C17 Ag4 -164.7(5) 2_765 2_665
Ag4 Ag5 C17 Ag4 15.3(5) . 2_665
Ag1 Ag5 C17 Ag4 41.1(3) 2_665 2_665
Ag5' Ag5 C17 Ag3 -56(3) . 2_765
C1 Ag5 C17 Ag3 -132.0(4) . 2_765
C25 Ag5 C17 Ag3 -9.6(4) 2_765 2_765
C9 Ag5 C17 Ag3 118.1(5) . 2_765
Ag2 Ag5 C17 Ag3 34.6(3) 2_765 2_765
Ag2 Ag5 C17 Ag3 82.1(3) . 2_765
Ag1 Ag5 C17 Ag3 137.9(3) . 2_765
Ag4 Ag5 C17 Ag3 -180.0(3) . 2_765
Ag1 Ag5 C17 Ag3 -154.3(3) 2_665 2_765
Ag2 C17 C18 C19 154(13) . .
Ag5' C17 C18 C19 -51(15) . .
Ag4 C17 C18 C19 -153(15) 2_665 .
Ag3 C17 C18 C19 33(15) 2_765 .
Ag5 C17 C18 C19 -57(15) . .
Ag2 C17 C18 Ag4 -53(2) . 2_665
Ag5' C17 C18 Ag4 102.1(8) . 2_665
Ag3 C17 C18 Ag4 -174.4(7) 2_765 2_665
Ag5 C17 C18 Ag4 95.6(7) . 2_665
C17 C18 C19 C20 -154(15) . .
Ag4 C18 C19 C20 54.4(12) 2_665 .
C17 C18 C19 C24 27(15) . .
Ag4 C18 C19 C24 -124.7(10) 2_665 .
C24 C19 C20 C21 0.0 . .
C18 C19 C20 C21 -179.1(13) . .
C19 C20 C21 C22 0.0 . .
C20 C21 C22 C23 0.0 . .
C21 C22 C23 C24 0.0 . .
C22 C23 C24 C19 0.0 . .
C20 C19 C24 C23 0.0 . .
C18 C19 C24 C23 179.0(13) . .
C17 Ag2 C25 C26 -12(7) . .
Ag3 Ag2 C25 C26 127(5) 2_765 .
Ag5 Ag2 C25 C26 126(5) 2_765 .
Ag5 Ag2 C25 C26 -145(5) . .
Ag3 Ag2 C25 C26 -148(5) . .
Ag4 Ag2 C25 C26 -46(5) 2_665 .
Ag5' Ag2 C25 C26 130(5) 2_765 .
Ag1 Ag2 C25 C26 -97(5) . .
Ag5' Ag2 C25 C26 -150(5) . .
C17 Ag2 C25 C26' 38(4) . .
Ag3 Ag2 C25 C26' 176.5(16) 2_765 .
Ag5 Ag2 C25 C26' 175.4(19) 2_765 .
Ag5 Ag2 C25 C26' -95.6(18) . .
Ag3 Ag2 C25 C26' -97.9(18) . .
Ag4 Ag2 C25 C26' 4.1(19) 2_665 .
Ag5' Ag2 C25 C26' 180(2) 2_765 .
Ag1 Ag2 C25 C26' -47.1(17) . .
Ag5' Ag2 C25 C26' -99.9(18) . .
C17 Ag2 C25 Ag5' -142(3) . 2_765
Ag3 Ag2 C25 Ag5' -3.4(6) 2_765 2_765
Ag5 Ag2 C25 Ag5' -4.5(5) 2_765 2_765
Ag5 Ag2 C25 Ag5' 84.5(6) . 2_765
Ag3 Ag2 C25 Ag5' 82.2(5) . 2_765
Ag4 Ag2 C25 Ag5' -175.8(3) 2_665 2_765
Ag1 Ag2 C25 Ag5' 133.0(4) . 2_765
Ag5' Ag2 C25 Ag5' 80.2(8) . 2_765
C17 Ag2 C25 Ag5 -137(3) . 2_765
Ag3 Ag2 C25 Ag5 1.2(6) 2_765 2_765
Ag5 Ag2 C25 Ag5 89.1(5) . 2_765
Ag3 Ag2 C25 Ag5 86.8(4) . 2_765
Ag4 Ag2 C25 Ag5 -171.3(3) 2_665 2_765
Ag5' Ag2 C25 Ag5 4.5(5) 2_765 2_765
Ag1 Ag2 C25 Ag5 137.5(4) . 2_765
Ag5' Ag2 C25 Ag5 84.7(6) . 2_765
C17 Ag2 C25 Ag3 136(3) . .
Ag3 Ag2 C25 Ag3 -85.6(4) 2_765 .
Ag5 Ag2 C25 Ag3 -86.8(4) 2_765 .
Ag5 Ag2 C25 Ag3 2.3(5) . .
Ag4 Ag2 C25 Ag3 102.0(3) 2_665 .
Ag5' Ag2 C25 Ag3 -82.2(5) 2_765 .
Ag1 Ag2 C25 Ag3 50.8(2) . .
Ag5' Ag2 C25 Ag3 -2.1(6) . .
O2 Ag3 C25 C26 6.9(14) . .
C9 Ag3 C25 C26 136.0(13) . .
C17 Ag3 C25 C26 -94.8(13) 2_765 .
C10 Ag3 C25 C26 138.4(13) . .
Ag5' Ag3 C25 C26 -98.6(14) 2_765 .
Ag2 Ag3 C25 C26 -138.3(13) 2_765 .
Ag2 Ag3 C25 C26 171.2(14) . .
Ag1 Ag3 C25 C26 118.3(13) . .
Ag5 Ag3 C25 C26 -105.3(14) 2_765 .
O2 Ag3 C25 C26' -33.7(14) . .
C9 Ag3 C25 C26' 95.4(14) . .
C17 Ag3 C25 C26' -135.5(14) 2_765 .
C10 Ag3 C25 C26' 97.7(15) . .
Ag5' Ag3 C25 C26' -139.2(16) 2_765 .
Ag2 Ag3 C25 C26' -178.9(14) 2_765 .
Ag2 Ag3 C25 C26' 130.5(15) . .
Ag1 Ag3 C25 C26' 77.6(14) . .
Ag5 Ag3 C25 C26' -146.0(15) 2_765 .
O2 Ag3 C25 Ag2 -164.2(4) . .
C9 Ag3 C25 Ag2 -35.2(6) . .
C17 Ag3 C25 Ag2 94.0(4) 2_765 .
C10 Ag3 C25 Ag2 -32.8(9) . .
Ag5' Ag3 C25 Ag2 90.2(6) 2_765 .
Ag2 Ag3 C25 Ag2 50.5(3) 2_765 .
Ag1 Ag3 C25 Ag2 -52.9(3) . .
Ag5 Ag3 C25 Ag2 83.5(4) 2_765 .
O2 Ag3 C25 Ag5' 105.5(6) . 2_765
C9 Ag3 C25 Ag5' -125.4(6) . 2_765
C17 Ag3 C25 Ag5' 3.8(6) 2_765 2_765
C10 Ag3 C25 Ag5' -123.0(8) . 2_765
Ag2 Ag3 C25 Ag5' -39.7(6) 2_765 2_765
Ag2 Ag3 C25 Ag5' -90.2(6) . 2_765
Ag1 Ag3 C25 Ag5' -143.1(6) . 2_765
Ag5 Ag3 C25 Ag5' -6.7(5) 2_765 2_765
O2 Ag3 C25 Ag5 112.3(5) . 2_765
C9 Ag3 C25 Ag5 -118.7(4) . 2_765
C17 Ag3 C25 Ag5 10.5(4) 2_765 2_765
C10 Ag3 C25 Ag5 -116.3(7) . 2_765
Ag5' Ag3 C25 Ag5 6.7(5) 2_765 2_765
Ag2 Ag3 C25 Ag5 -33.0(3) 2_765 2_765
Ag2 Ag3 C25 Ag5 -83.5(4) . 2_765
Ag1 Ag3 C25 Ag5 -136.4(3) . 2_765
C26' C25 C26 C27 -39(15) . .
Ag2 C25 C26 C27 24(20) . .
Ag5' C25 C26 C27 153(15) 2_765 .
Ag5 C25 C26 C27 147(15) 2_765 .
Ag3 C25 C26 C27 -121(15) . .
C26' C25 C26 Ag5' 168(2) . 2_765
Ag2 C25 C26 Ag5' -129(5) . 2_765
Ag5 C25 C26 Ag5' -6.0(5) 2_765 2_765
Ag3 C25 C26 Ag5' 85.2(8) . 2_765
C25 C26 C27 C28 -20(16) . .
Ag5' C26 C27 C28 130.0(17) 2_765 .
C25 C26 C27 C32 157(15) . .
Ag5' C26 C27 C32 -52(2) 2_765 .
C32 C27 C28 C29 0.0 . .
C26 C27 C28 C29 178(2) . .
C27 C28 C29 C30 0.0 . .
C27 C28 C29 C30 40(3) . 2_764
C28 C29 C30 C30 129(3) . 2_764
C28 C29 C30 C31 0.0 . .
C30 C29 C30 C31 -129(3) 2_764 .
C28 C29 C30 C29 129(5) . 2_764
C30 C29 C30 C29 0(2) 2_764 2_764
C30 C30 C31 C32 -122(4) 2_764 .
C29 C30 C31 C32 0.0 . .
C29 C30 C31 C32 -154(3) 2_764 .
C30 C31 C32 C27 0.0 . .
C28 C27 C32 C31 0.0 . .
C26 C27 C32 C31 -177.6(18) . .
C26 C25 C26' C27' 174(22) . .
Ag2 C25 C26' C27' 12(22) . .
Ag5' C25 C26' C27' -168(20) 2_765 .
Ag5 C25 C26' C27' -176(19) 2_765 .
Ag3 C25 C26' C27' -79(21) . .
C25 C26' C27' C28' -118(21) . .
C25 C26' C27' C32' 63(21) . .
C32' C27' C28' C29' 0.0 . .
C26' C27' C28' C29' -178.8(16) . .
C27' C28' C29' C30' 0.0 . .
C28' C29' C30' C31' 0.0 . .
C28' C29' C30' C30' -166(2) . 2_664
C29' C30' C31' C32' 0.0 . .
C30' C30' C31' C32' 157(4) 2_664 .
C30' C31' C32' C27' 0.0 . .
C28' C27' C32' C31' 0.0 . .
C26' C27' C32' C31' 178.7(17) . .
C1 Ag4 O1 S1' -82.1(17) . .
C17 Ag4 O1 S1' 51.7(17) 2_665 .
C18 Ag4 O1 S1' 77.3(17) 2_665 .
C9 Ag4 O1 S1' 172.1(16) . .
Ag1 Ag4 O1 S1' 140.9(15) . .
Ag1 Ag4 O1 S1' -42.6(18) 2_665 .
Ag2 Ag4 O1 S1' 9.7(17) 2_665 .
Ag5 Ag4 O1 S1' -132.1(16) . .
C1 Ag4 O1 S1 -31.0(11) . .
C17 Ag4 O1 S1 102.8(10) 2_665 .
C18 Ag4 O1 S1 128.4(10) 2_665 .
C9 Ag4 O1 S1 -136.9(9) . .
Ag1 Ag4 O1 S1 -168.0(6) . .
Ag1 Ag4 O1 S1 8.5(13) 2_665 .
Ag2 Ag4 O1 S1 60.7(10) 2_665 .
Ag5 Ag4 O1 S1 -81.1(10) . .
S1' O1 S1 C34 3(2) . .
Ag4 O1 S1 C34 -110.0(17) . .
S1' O1 S1 C33 -94(2) . .
Ag4 O1 S1 C33 153.2(18) . .
C9 Ag3 O2 S2 165.7(19) . .
C25 Ag3 O2 S2 -58(2) . .
C17 Ag3 O2 S2 43(2) 2_765 .
C10 Ag3 O2 S2 143.3(19) . .
Ag5' Ag3 O2 S2 -10(2) 2_765 .
Ag2 Ag3 O2 S2 61(2) 2_765 .
Ag2 Ag3 O2 S2 -77(2) . .
Ag1 Ag3 O2 S2 -148.5(19) . .
Ag5 Ag3 O2 S2 -9(2) 2_765 .
C9 Ag3 O2 S2' -38.5(12) . .
C25 Ag3 O2 S2' 97.8(11) . .
C17 Ag3 O2 S2' -160.8(11) 2_765 .
C10 Ag3 O2 S2' -60.9(11) . .
Ag5' Ag3 O2 S2' 146.0(10) 2_765 .
Ag2 Ag3 O2 S2' -143.3(9) 2_765 .
Ag2 Ag3 O2 S2' 79.0(12) . .
Ag1 Ag3 O2 S2' 7.2(12) . .
Ag5 Ag3 O2 S2' 146.4(10) 2_765 .
S2' O2 S2 C35 78(3) . .
Ag3 O2 S2 C35 -122(3) . .
S2' O2 S2 C36 -6(4) . .
Ag3 O2 S2 C36 154(4) . .
